Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this presentation? Why not share!

365 views

Published on

No Downloads

Total views

365

On SlideShare

0

From Embeds

0

Number of Embeds

4

Shares

0

Downloads

0

Comments

0

Likes

1

No embeds

No notes for slide

- 1. Chapter 3 Fibrous Piezoelectric Composites In the previous two chapters we presented some fundamental ideas about piezoelec- tric composites and their mathematical treatment, including the linear theory of piezoelectricity and the corresponding solution techniques. We now try to genera- lize these ideas to a range of fibrous composite problems such as piezoelectric fiber push-out and pull-out, stress and electric field transfer between fiber and matrix, debonding criteria for the fiber push-out test, effective material properties of com- posites, and solutions of piezoelectric composites with an elliptic fiber. All these topics are analyzed within the framework of linear theory of piezoelectric materials. 3.1 Introduction Piezoelectric fiber composites (PFCs), which comprise uniaxially aligned piezo- electric fibers embedded in a polymer matrix, have been widely used in recent years as transducers in applications such as sensors and actuators, sonar projectors, un- derwater use, medical ultrasonic imaging applications, and health monitoring sys- tems [1]. There are currently four leading industrial types of actuators that hold promise for intelligent structure applications. The first type is referred to as 1-3 composites, manufactured by Smart Material Corp. [2], and is typically used for ultrasonic and acoustic control applications. Active fiber composite (AFC) actuators were developed at MIT and were the first composite actuators to focus primarily on structural actuation [3-5]. Third, macrofiber composites (MFC) were developed at NASA Langley Research Center, also for structural actuation purposes [6]. Lastly, the idea of active composites fabricated with hollow cross-section fibers has been proposed [7] as a means of lowering the typically high voltages required to actuate AFCs and MFCs. It is noted that in the application of these smart composites, fracture induced by crack and interlaminar delimination is a major concern in many applications of PFCs, especially in aerospace where high structural reliability is required. Among various mechanisms contributing to the fracture resistance of composite materials, bridging by reinforcing fibers is considered to be of high interest because it pro- vides direct closure traction to the bridged crack [8]. To correlate the interfacial mechanical properties and experimental results and to study the mechanical beha- vior of the interface of PFCs, it is necessary to develop theoretical models (or em- pirical formulation) for analyzing stress and electric fields in piezoelectric fiber tests such as the push-out test and/or the pull-out test. Based on shear-lag assump- tions, the energy criterion and the Lamé solution for a 2D-axisymmetric problem, Q.-H. Qin, Advanced Mechanics of Piezoelectricity © Higher Education Press, Beijing and Springer-Verlag Berlin Heidelberg 2013
- 2. 54 Chapter 3 Fibrous Piezoelectric Composites many micromechanics models have been established over the past decades to pro- vide a theoretical basis for single fiber pull-out tests. The Gao-Mai-Cotterell model [9] and its modifications [10-12] have provided a theoretical basis for the analysis of stress distribution, interface debonding and friction for the pull-out test, using a fracture mechanics approach. Zhou et al. [13] reported a theoretical model for evaluation of the interfacial properties of ceramic matrix composites (with no pie- zoelectric effect) in push-out tests, based on the fracture mechanics approach. For PFC, Liu et al. [8] presented a theoretical model of fiber pull-out for simulation of the relationship between crack-opening and bridging stress using a shear stress cri- terion. Gu et al. [14] extended the model in [8] to include electric field input. Re- cently, Qin et al. [15] developed a theoretical model for analyzing piezoelectric be- havior in piezoelectric fiber push-out tests. Wang and Qin [16] presented a debond- ing criterion for determining interlaminar delimination during piezoelectric fiber push-out tests. Based on the model in [15] and some assumptions, Wang et al. [17] studied stress and electric field transfer in push-out tests under both electrical load- ing and mechanical loading. On the other hand, increasing applications of fibrous piezoelectric composites have naturally increased interest in the micromechanics modeling for such materials. Early reports of the effective material properties of isotropic reinforced solids are due to Hill [18], and a companion work in 1964 [19] on mechanical properties of fiber-strengthened materials. Hill’s report indicated that the overall elastic moduli of fibrous composites are connected by simple universal relations at given concentra- tions. Exact values of the effective properties can be determined when the phases have equal transverse shear modulus. In piezoelectric problems, Grekov et al. [20] studied the composite cylinder effective model for piezocomposites, Dunn and Taya [21] simplified the piezoelectric Eshelby’s tensors of the elliptic fiber problem and put them in explicit form instead of elliptic integrals, and then they extended the dilute, self-consistent, Mori-Tanaka and differential micromechanics methods to cover piezoelectric composites. Schulgasser [22] found that the effective constants of a two-phase fibrous piezoelectric composite are connected by simple relations. Ben- veniste and Dvorak [23] showed that in such composites, uniform fields can be generated by certain loading conditions. The concept of uniform fields was further elaborated by Benveniste [24,25] in two-, three-, and four-phase composites with cylindrical microstructures. Chen [26] presented a number of exact results for over- all moduli of a piezoelectric composite consisting of many perfectly-bonded phases of cylindrical shape. Mallik and Ray [27] reported improvement of the effective material coefficient of piezoelectric fiberreinforced composites by assuming the same electricfieldinbothmatrixandfiberphases.HuangandKuo[28]directlyextendedthe Eshelby type equivalent inclusion method to piezomagnetic composites and proposed an analogous simplification of Eshelby’s tensors [29]. Jiang et al. [30,31] presented a three-phase confocal elliptical model, in which the generalized self-consistent method
- 3. 3.2 Basic formulations for fiber push-out and pull-out tests 55 forpiezocompositeswasdevelopedasforthermo-electro-magneto-elasticcomposites. Recently, Tong et al. [32] presented a three-phase model under in-plane mechanical load coupling with thermo-electro- magnetical loads. Kumar and Chakraborty [33] developed an effective coupled thermo-electro-mechanical model of piezoelectric fiber reinforced composite using an approach based on strength of materials . This chapter, however, only includes most of the results appearing in [8,14-17,24-26,34,35]. 3.2 Basic formulations for fiber push-out and pull-out tests The geometric configuration of the micromechanical model used in the single pie- zoelectric fiber pull-out test and push-out test is shown in Fig. 3.1 [8,16], with an interfacial debonding crack of length l. A piezoelectric fiber polarized in the axial direction with radius a and length L is embedded at the centre of a coaxial cylindri- cal shell of epoxy matrix with external radius b. A uniform stress (tension in pull-out test and pressure in push-out test) and an electrical loading a a are applied at the end of the fiber ( ). The piezoelectric fiber is considered transversely isotropic and the epoxy is isotropic. In the following, basic formulations for the model shown in Fig. 3.1 are presented in order to establish notation and to provide a common source for reference in later sections of this chapter. 0z Fig. 3.1 Mechanics model of PFCs in (a) fiber pull-out test, (b) fiber push-out test. Based on linear piezoelectric theory, the relationship between strains and stresses is expressed as [36]
- 4. 56 Chapter 3 Fibrous Piezoelectric Composites f f 11 12 13 13 f f 12 11 13 13 f f 13 13 33 33 f f 55 15 0 0 0 0 0 0 0 0 0 02 rr rr r zzz zz rz rz f f f g f f f g D f f f g D f g (3.1) f f 15 11 f 13 13 33 33 f 0 0 0 0 0 0 rr r r z zzz rz gE D g g gE D (3.2) for pure mechanical loading, and f f 11 12 13 13 f f 12 11 13 13 f f 13 13 33 33 f f 55 15 0 0 0 0 0 0 0 0 0 02 rr rr r zzz zz rz rz f f f d f f f d E f f f d E f d (3.3) f f 15 11 f 13 13 33 33 f 0 0 0 0 0 0 rr r r z zzz rz dD E d d dD E (3.4) for electromechanical loading [17], where the superscripts “m” (in Eq. (3.5) below) and “f ” refer to the variable associated with “matrix” and “fiber” respectively. In the above formula, (dij, gij) and ( ,ij ij ) are piezoelectric coefficient and dielectric constants, ijf are components of elastic compliance. The constitutive relations of the elastic matrix are given by m m m m m m m m 1 0 1 01 1 0 0 0 0 2(1 )2 r rr z zz rz rz E (3.5) The general equilibrium equations for the fiber-matrix system are given by 0 j j j zz rz rz z r r (3.6) 0 j jj j rrrr rz r z r (3.7)
- 5. 3.2 Basic formulations for fiber push-out and pull-out tests 57 0r r zD D D r r z (3.8) where j=m, f. Making use of Eqs. (3.6) and (3.7), the equilibrium between the axial stress and the interfacial stress can be expressed as f m1 a zz zz (3.9) m d 2 ( ) d zz i z z a (3.10) f d 2 ( ) d zz i z z a (3.11) where (3.12)2 2 2 /( )a b a and all stresses appearing in Eqs. (3.9)-(3.11) are taken to be the corresponding average values with respect to the cross section. Substituting Eqs. (3.10) and (3.11) into Eq. (3.6) yields the shear stresses in the fiber and the matrix as follows: f ( )rz i r z a (3.13) 2 2 m ( ) ( )rz i b r z ar (3.14) The electric field, Ei, is defined in Eq. (1.2), i.e., ,r zE E r z (3.15) To simplify the derivation of the theoretical model and without loss of generality, the axial stresses f zz and m zz are assumed to be functions of z only, and the electric potential which is caused by elastic deformation of the fiber is also inde- pendent of r [15], i.e., (3.16)f f m m ( ), ( ), ( )zz zz zz zzz z z a z For a long fiber ( ) polarized in the z-direction embedded in a relatively large matrix, this assumption is appropriate, and because of the transversely iso- tropic property of the piezoelectric fiber the following assumption is still accept- able: L (3.17)f f ( ) ) ( )rr iz z q
- 6. 58 Chapter 3 Fibrous Piezoelectric Composites where is the interfacial radial stress induced by Poisson contraction between the fiber and the matrix or/and applied electric field. Using Eqs. ( )iq z (3.2), (3.8), (3.15), and (3.16), the electric displacements in the fiber can be expressed in terms of fiber stresses as f f f 15 15, f z zz r rzD d D d (3.18) Substituting Eq. (3.17) into Eq. (3.3), we obtain (3.19)f f rr Using the strain-displacement relationships in the axi-symmetric problem andr r rr u u r r (3.20) we have r ru u r r (3.21) where ur is the radial displacement. The solution of Eq. (3.21) shows that are independent of the coordinate r. Thus, it can be concluded that the axial electric field Ez is also independent of the variable r [14]. Integrating Eq. andr (3.15)2 with respect to z, we obtain 1 2( , ) ( ) ( )r z f r f z (3.22) Substituting Eq. (3.22) into Eqs. (3.4) and (3.8), we have 1( ) lnf r A r B (3.23) f 2 13 33 15 33 1 ( ) [2 ( ) ( ) ( )]di zzf z d q z d d z z Cz D (3.24) in which A, B, C, and D are integral constants and, in general, it is assumed that B=D=0 because there is no effect on Ei and Di after the differential operation [14]. Note that f1(r) approaches infinity when r tends to 0, which implies A=0. C can be determined by using the electric boundary condition, say, 0z zD 0D (3.25) where D0 is the electric displacement applied at the end of the fiber. Making use of Eqs. (3.4) and (3.24), C can be determined as (3.26)15 0aC d D It can be seen from Eq. (3.24) that the electric potential is also independent of
- 7. 3.3 Piezoelectric fiber pull-out 59 the variable r. In the frictional sliding interface, , the interfacial shear stress i is go- verned by Coulomb’s friction law [36]. That is, 0 z l 0( ) ( )i z q qi z (3.27) in which is a constant coefficient of friction and is the residual fiber clamp- ing (compressive) stress in the radial direction caused by matrix shrinkage and dif- ferential thermal contraction of the constituents upon cooling from the processing temperature. 0q The outer boundary conditions of the matrix are given by m 0r r b , m 0rz r b (3.28) At the interface, the radial stresses and displacements of the fiber and matrix satisfy m f m f ,rr rr i r r r a r a r a r a q u u (3.29) At the bonded interface, , the continuity of axial deformations re- quires that l z L m f z z r a r a u u (3.30) The remaining task is to derive the differential equation for f zz and radial stress due to elastic deformation in composites with a perfectly bonded interface or in the frictional sliding process after the interface is completely debonded. The de- tailed derivations for these two processes are provided in the following three sec- tions. ( )iq z 3.3 Piezoelectric fiber pull-out In this section a theoretical model presented in [8,14] is introduced for investigating the interaction between fiber deformation, pull-out stress and electric fields. The model can be used to examine stress distributions in the fiber under both mechani- cal and electric loads. In the following, the solutions for elastic and electric fields in both bonded region and frictional sliding region are presented. 3.3.1 Relationships between matrix stresses and interfacial shear stress The radial and hoop stresses in the matrix can be expressed in terms of
- 8. 60 Chapter 3 Fibrous Piezoelectric Composites ( ) and ( )i iz q z by way of the strain compatibility and equilibrium equations. Noting that by assumption, the axial stress is dependent on z only, the strain com- patibility equation can be written as [14] m m m m 1 rr rr r r r (3.31) Substituting Eq. (3.31) into Eq. (3.7) we obtain 2 m m ( ) ( ) 2 (1 ) i rr zr F z a z (3.32) where the function F(z) is to be determined by the boundary conditions. In the pull-out test, the boundary conditions for radial and hoop stresses can be assumed to be m ( ) and 0rr r a i rr r bq z m (3.33) Thus, the solutions for radial and hoop stresses can be written as m 1 2 m 3 4 d ( ) ( , ) ( ) ( ) ( ) , d d ( ) ( , ) ( ) ( ) ( ) d i rr i i rr i z r z p r q z p r z z r z p r q z p r z (3.34) where 2 1 2 ( ) 1 b p r r , 2 2 2 2 2 1 22 2 ( ) 2 ln ln 1 1 ( ) , 4 b b b b p r b r a a r a r r 2 2 3 2 2 2 21 4 2 2 2 2 22 2 ( ) 1 , ( ) 2 ln ln 1 2( ) 4 1 ( ) 4 4 b p r r b b b p r b r b a r a r b r a b a r 2 with 1 21 , (3 )/ 2
- 9. 3.3 Piezoelectric fiber pull-out 61 3.3.2 Solution for bonded region In the solution for the bonded region, the following continuity conditions at r=a can be used: (3.35)f m f ,r r z zu u u um Making use of Eqs. (3.9) and (3.17) and the continuity condition (3.35), we have f f 2 3 2 1 1 ( )d ( ) d( ) i a z z i z 3g g a zq z a g a (3.36) where 2 13 13 33 15 13 0 15 1 11 12 2 33 3 33 33 33 3 4 1 2 3 2 ( ) ( , , ( ) ( ) , , ad d d d d D a f f a f a p a p a g g g E E E )d Combining Eqs. (3.9), (3.11), (3.35) and (3.36) with axial displacements and stresses, a second-order differential equation of the axial stress in the fiber is ob- tained: 2 f f 1 22 d 0 d zz zzA A z (3.37) where 1 1 2 2 1 1 2 1 1 2 1 1 1 2 3 1 1 2 3 / , / ( ) ( ) , 2 ( )( ) ( )( A M M A M M a M b h g a g h ),M b h a g a g b h 2 1 1 3 3 1 1 3 3( )( ) ( )(a aM b h a g a g b h ) 13 33 33 33 15 33 0 15 1 13 2 33 3 33 33 33 2 ( ) ( 2 , , ad d d d d d D d b f b f b ) 3 4 1 2 [ ( ) 1] ( ) 1 , , p a p a h h E E 3h E For the case of the pull-out test shown in Fig. 3.1(a), the boundary conditions are (3.38)f f (0) , ( ) 0zz a zz L
- 10. 62 Chapter 3 Fibrous Piezoelectric Composites The solution to Eq. (3.37) is then obtained as (3.39)f 1 2 2( ) /z z zz z k e k e A A1 where 2 1 1 2 1 2 2 2 1 , (1 ) 1 1 (1 ) 1 L L L aL L aL Ae A k e e Ae A k e Ae , As mentioned in [14], based on Eq. (3.39), the interfacial shear stress can be evaluated from Eq. (3.11). Then the interfacial normal stress qi(z) can be determined from Eq. (3.36). Meanwhile the electric potential can be calculated from Eqs. (3.22)-(3.24) with the proper boundary conditions, such as ( )i z ( ) 0L . In this chapter, the yielding shear stress, , is taken as the maximum shear stress at which debonding starts along the interface between fiber and matrix, if the shear stress at the interface reaches . y y 3.3.3 Solution for debonded region In the case of friction sliding, the interfacial shear stress is determined from Cou- lomb’s friction law (3.27). Making use of Eqs. (3.9), (3.11), (3.27), and (3.36), we obtain 2 f f f 1 2 32 d d 0 dd zz zz zzB B B zz 3) 0 ]D 2 (3.40) where / ( 1,2,i iB N N i 2 1 1 1 2 2 3 3 3 3 1 1 / 2, ( ) / 2, ( ), [( ) ( )a N a g N a a g N a g N a g a g Equation (3.40) can be solved for fiber stress using the following boundary conditions [14]: (3.41)f f (0) , ( ) 0zz a zz L l The solution to Eqs. (3.40) and (3.41) can, then, be written as (3.42)1 2f 3 4 3( ) /z z zz z k e k e B B where
- 11. 3.4 Piezoelectric fiber push-out 63 2 1 1 2 1,2 4 , 2 B B B 1 2 2 1 2 1 1 2 ( ) ( ) ( )3 3 ( )( ) 2 ( ) 3 4 ( )( ) 2 (1 ) , 1 1 (1 ) 1 L l L l L l aL l L l aL l Be k e e Be B k e Be 3.3.4 Numerical results To illustrate applications of the theoretical model described above, numerical results are presented for a piezoelectric/epoxy system, of which the material properties are [8]: E=3 GPa, =0.4, 11f = 0.019 GPa–1 , 33f = 0.015 GPa–1 , 12f =–0.005 7 GPa–1 , 13f =–0.004 5 GPa–1 , 55f = 0.039 GPa–1 . The radii of the matrix and fiber are 3 mm and 0.065 mm, respectively. The piezoelectric parameters of the fiber are given by: d33=390 10–12 m/V, d13 =–d15=–190 10–12 m/V, 11=40 10–9 N/V2 , 33=16.25 10–9 N/V2 . The interfacial properties are approximately evaluated as s=0.04 GPa and =0.8. The initial thermal stress q0 is taken to be 0. Figure 3.2 shows the stress and electric fields in the piezoelectric fiber, where the debonding length is 0.4 mm. In the debonded region ( ), both the fiber axial stress and the electric field are nearly constant. In the bonded area, their values reduce rapidly. In the boundary between the bonded and debonded regions, Ez has a significant increment. 0 0z .4 Fig. 3.2 Stress and electric fields in the piezoelectric fiber. 3.4 Piezoelectric fiber push-out In the previous section we presented a theoretical model for simulating the me-
- 12. 64 Chapter 3 Fibrous Piezoelectric Composites chanical behavior of PFCs in a pull-out test. Extension to the case of PFCs in the push-out test is described in this section. The mechanics model to be employed is shown in Fig. 3.1(b). Using the piezoelectric fiber push-out model presented in this section, the effect of piezoelectric constant and embedded fiber length on the me- chanical behavior of fiber composites is investigated. The results show that there is a significant effect of the piezoelectric parameter and embedded fiber length on stress transfer, electric field distribution and load-displacement curve of the fric- tional sliding process. 3.4.1 Stress transfer in the bonded region Stress transfer is of fundamental importance in determining the mechanical proper- ties of fiber-reinforced composite materials. For the interface in PFCs, stress trans- fer is affected by the piezoelectric coefficient in addition to the micromechanical properties. In the following, the derivation of a second-order differential equation of f zz presented in [15,17] is briefly reviewed. Consider the mechanics model shown in Fig. 3.1(b). The inner and outer boun- dary conditions of the matrix are given by (3.43)m m m m ( , ) ( ), ( , ) ( ), ( , ) 0, ( , ) 0rr i rz i rr rza z q z a z z b z b z Then from Eqs. (3.14) and (3.43), we obtain [37] m 2 2 2 2 2 2 2 1 2 d ( , ) ( )( 1) 4 d 2 ln( ) ( 1)ln( ) ( )(1 ) i rr ir z q z b r a z b r b b r b a b r a r2 2 (3.44) m 2 2 2 1 2 2 2 2 2 2 2 2 2 1 2 d ( , ) ( )(1 ) 2 ln ( ) 4 d ( 1)ln ( ) 4 2 ( ) ( )(1 i ir z q z r b b r b a z b r b a b b r b r a r ) (3.45) Substituting Eqs. (3.44) and (3.45) into Eq. (3.5) yields m 2 2 m 2 1 2 2 2 2 2 1 2 d ( ) 1 1 2 (1 ) ln 4 d ln 2 ln 1 1 ir i z Eu q z b r b r b r a z b a b b a b r b r a r2 2 2 2 2 2 2 2 2 2 11 4 2b r a r b b r (3.46)
- 13. 3.4 Piezoelectric fiber push-out 65 m m 2 1 d 2 ( ) 2 2 ln ln 4 d iz i z E u q z b r b b a z a z 2 2 2 2 2 1 22b r b a b (3.47) For a fully bonded interface, the continuity conditions of axial and radial defor- mation between fiber and matrix are given in Eqs. (3.29) and (3.30). From Eqs. (3.1), (3.30) and (3.47), the radial stress of the fiber is obtained as f 33 33 15 13 2 2 2 2 2 2 1 1 2 d1 ( ) / / 2 4 d2( / ) 2 (1 )ln ( ) 2 ( ) i i a zq z E E f g d Ea zf E b a b b a b a b (3.48) Then, combining Eqs. (3.1), (3.29), (3.46), and (3.48) yields the differential equation of f z in the form 2 f f 1 22 d ( ) ( ) d z z a z A z A z (3.49) where 1A and 2A are two constants: 13 31 15 1 33 33 15 1 1 1 2 / ( / ( 2 / ) 8 E f g d B E f g d A C B C E ) (3.50) 1 2 1 1 2 / / ( 2 / 8 E B E A C B C E) (3.51) with 2 2 12 11 1 13 ( 1) ( ) (1 ) / 2( / ) f f b Ea B f E E (3.52) 2 2 1 1 1 2 2 2 2 2 2 11 1 2 (1 )(1 )ln( ) / 2 ln( )( 1) ( 2 ( ) / 4 / 2 ( ) C b a b E b b a b Ea a b E b E s b a 2 2 ) (3.53) 2 2 2 2 2 1 1 22 (1 )ln( ) ( ) 2 (C b a b b a b a b2 2 ) (3.54) 1 2(1 ) (3.55) 2 (1 ) 1 (3.56) Using the stress boundary conditions
- 14. 66 Chapter 3 Fibrous Piezoelectric Composites (3.57)f f (0) , ( ) 0z a z L The axial stress in the piezoelectric fiber is given by f 2 1 1 2 1 1 ( ) sinh( ) cosh( )z a A z K A z K A z A (3.58) where 1K and 2K are defined by 2 2 1 1 1 1 1 1 cosh( ) sinh( ) a A A A L A A K A L (3.59) 2 2 1 1 a A K A (3.60) In addition, using Eqs. (3.6), (3.7), and (3.17), can be expressed as( )iq z 2 f f 1 2 3 2 d ( ) d z i a zq z N N N z (3.61) where (i=1,2,3) are given byiN 33 33 15 2 1 2 13 13 / , , 42( ) 2( / ) E f g d C N N N EEf f E 3 (3.62) From Eqs. (3.2), (3.18), (3.58), and (3.61), the electric field zE can be calcu- lated by f15 31 33 33 ( ) 2 ( ) ( )z i d E z g q z g zzz (3.63) 3.4.2 Frictional sliding Once the interface debonds completely, the frictional sliding of the fiber out of the surrounding matrix will begin, which is the last stage of the push-out process. To better characterize this stage, theoretical analysis was conducted with the microme- chanical model shown in Fig. 3.3. For the sake of simplicity, we assume a small elastic deformation and a large displacement at the fiber-loaded end during sliding. Therefore, the elastic deforma- tion of the fiber can be neglected, and the fiber axial displacement approximately equals the fiber sliding distance s, that is, s . The governing equation for f z in this case can be derived in a manner similar
- 15. 3.4 Piezoelectric fiber push-out 67 to the mathematical operation for Eq. (3.49). In fact, from the continuity condition of radial displacement (3.29) and Eqs. (3.6), (3.14), and (3.17), we have f13 13 31 15 1 1 1 / ( ) 4 d i i a z f f E g d C q z D D a 1 d D z (3.64) Fig. 3.3 A fiber-matrix cylinder model for frictional sliding in the push-out test. Substituting Eq. (3.64) into Eq. (3.27) yields 2 f f f 1 22 d ( ) d ( ) ( ) dd z z z z z Q Q z zz 3Q (3.65) where (i=1,2,3) are given byiQ 1 1 1 4aD Q C (3.66) 13 31 15 2 1 8( / )E f g d Q C (3.67) 1 3 1 1 8 a D Q C D E 0q (3.68) with 2 2 1 12 11 ( 1) ( ) (1 ) /D f f b Ea E (3.69) Using the stress boundary conditions (3.70)f f ( ) , ( ) 0z a zs L The solution to Eq. (3.65) is obtained as 1 2f 3 3 4 2 ( ) z z z Q z K e K e Q (3.71) where s is the fiber sliding distance (see Fig. 3.3) and are given by3 4 1, , ,K K 2
- 16. 68 Chapter 3 Fibrous Piezoelectric Composites 3 3 3 3 aK Q m n , (3.72)4 3 4 4 aK Q m n 2 1 1 1 1 1 4 2 2 Q Q Q2 , 2 2 1 1 1 1 4 2 2 Q Q Q2 (3.73) with 2 2 1 2 1 2 3 2 ( ) L s L s s L e e m Q e e , 1 1 1 2 1 2 4 2 ( ) s L L s s L e e m Q e e (3.74) 2 1 2 1 2 3 L L s s L e n e e , 1 1 2 1 2 4 L L s s L e n e e (3.75) In the process, the interfacial shear stress is governed by Coulomb’s frictional law given in Eq. (3.27). Noting that fiber and matrix maintain contact in the radial direction, we have (3.76)f m ( , ) ( , )r ru a z u a z Then, the radial normal stress can be expressed as 2 f 1 2 3 2 d ( ) d z i aq z M M M z (3.77) where iM (i=1,2,3) are given by 1 1 ,M ED 13 31 15 2 1 / E f g d M D , 1 3 18 C M D (3.78) Using Eqs. (3.2), (3.18), (3.71), and (3.77), the electric field can be obtained as f15 31 33 33 ( ) 2 ( ) ( )z i d E z g q z g zz (3.79) Noting that the sum of the radial normal stress of the fiber should be negative, and the fiber and matrix can contact each other during the fiber sliding process, the radial stress must satisfy the expression (3.80)0 ( ) 0iq q z According to the distribution of the fiber stress fields in the push-out test, the axial stress reaches its maximum value at the fiber-loaded end ( , and s is defined in Fig. 3.3), while the interfacial shear stress reaches its minimum value at the same location. Then Eq. z s 0s (3.80) yields (3.81)0 ( ) 0iq q s Therefore the relationship between the applied stress and the axial dis-a
- 17. 3.4 Piezoelectric fiber push-out 69 placement ( s) at the fiber-loaded end can be given as 1 2 1 2 1 2 0 3 1 4 2 2 2 2 2 21 15 1 3 1 4 2 3 1 4 2 1 1 1 (1 ) ( ) ( ) 8 s s a 13 3 s s s s q m e m e d C m e m e n e n e D ED D f g (3.82) 3.4.3 PFC push-out driven by electrical and mechanical loading The formulation presented above can handle push-out problems under mechanical loading only. In the following, discussion of PFC push-out testing subjected to both mechanical and electric loading is presented. Consider now the electrical boundary conditions at the ends of the piezoelectric fiber: (0) , ( ) 0V L (3.83) From Eq. (3.24), we have f 13 33 15 0 33 1 2 ( ) ( ) ( ) d ( L i z )C d q z d d z z D V L L V (3.84) Following the procedure in Subsections 3.4.1 and 3.4.2, solutions of the stress fields in the bonded region ( ) can be written asl z L m ( ) 1 exp( )z az z (3.85) f ( ) 1 exp( )z a az z (3.86) * ( ) ( )exp( ) 2 i a a z z (3.87) f m 13 13 33 15 33 13 2 11 12 13 33 ( ) / ( ) ( ) ( ) ( 2 / ) 1 2 zz zE f d d d z z Ed C E f f d iq z (3.88) in which 13 13 33 15 33 13 13 33 15 33 ( )/ ( ) / E f d d d E f d d d (3.89) * 0q q (3.90) 2 a (3.91)
- 18. 70 Chapter 3 Fibrous Piezoelectric Composites 13 13 33 15 33 2 11 12 13 33 ( ) / ( 2 / ) 1 2 E f d d d E f f d (3.92) 13 2 11 12 13 33( 2 / ) 1 2 Ed C q E f f d (3.93) The solutions of the stress fields in the bonded region ( ) are obtained asl z L 2 2 1 1 1f 1 2 11 sinh ( ) sinh ( ) ( ) sinh ( ) a l a z a A A A L z A l z A A A z AA L l (3.94) 2 2 1 1 12m 1 1 1 sinh ( ) sinh ( ) 1( ) sinh ( ) a l a z a A A A L z A l z AA A z A A L l (3.95) 2 2 1 1 1 1 1 cosh ( ) cosh ( ) ( ) 2sinh ( ) a l a i A A a A L z A A z A L l A l z (3.96) where f ( ) 1 exp( )l zz a a l l (3.97) 33 33 33 15 33 13 13 33 33 1 2 2 2 ( ) / 2 ( (1 ) 2 ln( / ) E f d d d Ef Ed d A b b a a / ) (3.98) 13 13 33 33 * 13 13 33 33 33 2 2 2 2( / )( 1) 2 2 / (1 ) 2 ln( / ) a Ef Ed d E f d d q Ed C A b b a a a (3.99) The electrical field zE in both the debonded and bonded regions is given as f 13 33 15 33 1 2 ( ) ( ) ( )z i zE d q z d d z C (3.100) 3.4.4 Numerical assessment To illustrate applications of the proposed theoretical model and to reveal the effects
- 19. 3.4 Piezoelectric fiber push-out 71 of the electromechanical coupling on stress transfer behavior, numerical results are presented for a piezoceramic fiber/epoxy matrix system subjected to a push-out load. The material parameters are assumed to be the same as those used in Subsection 3.3.4. The radii of fiber and matrix are: The residual fiber clamping stress in radial direction is assumed to be –0.01 GPa and 0.065 mm, 3 mm,a b mm.L 0.8 l 0.6 mm ( 0 for fully bonded fiber), and 2l 0q [15,17]. Figures 3.4(a)-(d) shows the distribution of stresses and electric field as func- tions of the dimensionless axial distance z/L for a partially debonded piezoelectric composite system subject to a constant external stress GPa in the fiber push-out test. For comparison and illustration of the effect of electromechanical coupling on stress transfer behavior, the corresponding distribution of stresses for a non-piezoelectric fiber composite (NPFC) is also plotted in Fig. 3.4. It is found that the curves for PFC and NPFC have similar shapes. When subjected to applied stress of same value, the axial stress 1.5a f z in PFC is smaller than that in NPFC (Fig. 3.4(a)). It can also be seen from Figs. 3.4(a) and 3.4(c) that both axial and radial stresses in the fiber gradually decrease as increases. Figure. 3.4(c) demon- strates that there is a larger radial stress in the PFC and it decays more rapidly than that in NPFC, which leads to a larger interface shear stress in the debonded region /z L Fig. 3.4 Plot of (a) fiber axial stress, (b) interface shear stress, (c) fiber radial stress, (d) electric field for the piezoelectric fiber push-out under mechanical loading.
- 20. 72 Chapter 3 Fibrous Piezoelectric Composites of PFC in Fig. 3.4(b) due to the Coulomb friction law (3.27). This phenomenon can be attributed to the piezoelectric effect in piezoelectric fiber; a larger applied stress is required in PFC to produce the same axial stress as in NPFC. The difference in the stress fields between these two composite systems is controlled by piezoelectric coefficients, which were investigated in [15] for fully bonded composites. When the piezoelectric coefficients and dielectric constants are set as zero, piezoelectric fiber degenerates to non-piezoelectric fiber. Figure 3.4(d) shows the variation of electri- cal field as a function of axial distance z/L. The variation of zE with z/L is very simi- lar to that of the fiber axial stress. Figures 3.5(a)-(d) shows the distribution of stresses and electric field as func- tions of dimensionless axial distance z/L for a partially debonded piezoelectric composite system subject to electrical loading and a constant external stress GPa in the fiber push-out test. In order to study the effect of positive and negative electric loading on stress transfer, electric potentials of 5 000 V, 0 V, and –5 000 V are applied at the end of piezoelectric fiber (z = 0). Figure 3.5(a) shows that the fiber axial stress decays more rapidly under negative electric potential than under positive electric potential. It can also be seen from Fig. 3.5(c) that negative electric potential leads to a larger radial stress in the piezoelectric fiber than applied positive electric potential, whose positive electric potential accordingly causes a 1.5a Fig. 3.5 Plot of (a) fiber axial stress, (b) interface shear stress, (c) fiber radial stress, (d) electric field for the piezoelectric fiber push-out under electrical and mechanical loading.
- 21. 3.4 Piezoelectric fiber push-out 73 larger interface frictional shear stress in debonded region in Fig. 3.5(b). This is be- cause when piezoelectric fiber is subjected to an electric potential applied parallel to the polarization direction, expansion occurs in the same direction and shrinkage occurs in the transverse direction [38]. For a positive applied electric potential, the hoop stress developed is in compression, while for a negative applied electric po- tential, the hoop stress developed is in tension. In Fig. 3.5(d), the distribution of electric field in the piezoelectric fiber is plotted via z/L, and it depends heavily on the applied electric field. Figures 3.6-3.11 apply to problems with fully bonded fiber. Figures 3.6 and 3.7 present the distribution of fiber axial stress and interfacial shear stress at the first stage of push-out for different embedded fiber lengths. At the fiber end ( ), the applied stress is given by GPa. It is evident that the stress distribu- tion in the piezoelectric fiber is similar to that in conventional material fiber such as carbon fiber. The fiber axial stress decays rapidly near the fiber-loaded end and the rate of decay varies with the embedded fiber length. The curves in Fig. 3.7 show clearly that the maximum interfacial stress is not very sensitive to variation of fiber length when , and the interfacial stress remains almost constant when , which is quite similar to the finding in [37]. / 0z L 0.05a 2 mmL / 0.z L 6 Fig. 3.6 The distribution of fiber axial stress in fully bonded interfaces of different lengths (applied load stress is –0.05 ). f ( )zz z aa GP To study the effect of the piezoelectric parameter and electro-mechanical coupling on stress transfer, stress distribution is plotted in Figs. 3.8 and 3.9 for both non-piezolectric fiber and piezoelectric fiber with different where the fiber length mm. Figure 3.8 shows that axial stress decreases along with in- crease in the piezoelectric constant , i.e., axial stress will be smaller at any given position z/L for a larger value of . Axial stresses decay more rapidly in piezoelectric fiber than in non-piezoelectric fiber. The situation in Fig. 3.9 is 15d 2.0L 15d 15d
- 22. 74 Chapter 3 Fibrous Piezoelectric Composites slightly different. There is a critical location at which has no effect on interfacial shear stress. It is evident from Fig. 3.9 that shear stress will increase when z<zc and decrease when z>zc , along with an increase in the value of . This phenomenon indicates that the higher the value of , the higher the rate of decrease in both axial and shear stress. A comparison of the shear stress dis- tributions in piezoelectric and non-piezoelectric fiber is also made and plotted in Fig. 3.9, and their significant difference is observed. c / 0.2z L 4 15d 15d 15d Fig. 3.7 The distribution of interfacial shear stress in fully bonded interfaces of different lengths (applied load stress is –0.05 ). ( )i z GPaa Fig. 3.8 The distribution of fiber axial stress in a fully bonded region (applied load stress is –0.05 and d ). f ( )zz z 12 m/V10a GPa 15 190 Because of the piezoelectric effect, an electric field exists in the fiber. The dis- tribution of the electric field in axial direction zE is shown Figs. 3.10 and 3.11. It can be seen from these two figures that the distribution of the electric field and the effect of the fiber length and the parameter are quite similar to those of the15d
- 23. 3.4 Piezoelectric fiber push-out 75 stress field (Figs. 3.6-3.9). Fig. 3.9 The distribution of interfacial shear stress in a fully bonded region (applied load stress is –0.05 and ). ( )i z 12 m/Va GPa 15 190 10d Fig. 3.10 The distribution of electric fields in piezoelectric fiber for different embedded lengths (applied load stress is –0.05 and ).a GPa 12 15 190 10 m/Vd Fig. 3.11 The distribution of electric field in a piezoelectric fiber for different values of (applied load stress is –0.05 GP and ).15d a a 12 15 190 10 m/Vd
- 24. 76 Chapter 3 Fibrous Piezoelectric Composites 3.5 Interfacial debonding criterion In the previous two sections theoretical models were described for simulating fiber pull-out and push-out processes. A debonding criterion for identifying interfacial delimination during fiber push-out testing of PFC is introduced in this section. The debonding criterion can be used for investigating the debonding process of piezo- electric fiber in the push-out test under combined electrical and mechanical loading. The description in this section is based on the results presented in [16]. Unlike in NPFCs, there are electrical fields induced by the piezoelectric effect or inverse-piezoelectric effect of PFCs. Owing to this phenomenon, the debonding criterion for NPFCs is not directly applicable. To incorporate the piezoelectric effect in the debonding criterion we consider a cracked piezoelectric elastic body of vol- ume V in which traction P, frictional stress t, and the surface electrical charge are applied. , and are the corresponding surfaces respectively, as shown in Fig. 3.12. For the sake of simplicity, the matrix is assumed to be a piezo- electric material whose piezoelectric coefficients and dielectric constants equal zero. In our analysis, the debonding region is taken to be a crack (see Fig. 3.12). PS tS S Fig. 3.12 A piezoelectric elastic body with a frictional crack under electromechanical loading. Based on the principle of energy balance, the variation of energy in the piezo- electric system for crack growth dA along the friction surface under electro- mechanical loading is (3.101)fd d dcG A W where is fracture energy, is the work done by friction stress during crack growth, cG fW (3.102)f 0( ) d TS W t t v S and is the generalized mechanical and electrical energy stored inside the pie-
- 25. 3.5 Interfacial debonding criterion 77 zoelectric body: 0 0 1 ( ) : ( )d 2 e e s s 0 0 1 ( ) : ( )d d 2 PS S D D E E Pu S Sd (3.103) in which is the relative slip of crack surfaces and is the tangential compo- nent of pre-stress (or initial stress) on the crack surfaces. v 0t 0s , , e0, and E0 are selfequilibrium initial stress, electrical displacement, strain, and electrical field re- spectively, and 0D 0s s and balance the applied loads.0D D Using the basic theory of piezoelectricity (3.1)-(3.8), one can easily prove the corresponding reciprocal principle of work and the principle of virtual work for piezoelectric material: 1 2 1 2 1 2 2 1 2 1 2 1 d d d d di i i i i i i it u f u t u f u d (3.104) d d d d ( t i i i i ij ij i it u t u q D E )d (3.105) Using the two principles (3.104) and (3.105) and following a method similar to that employed for fiber pull-out analysis [39], it can be proved that against the incremental debonding length, l, is equal to the energy release rate for the debonded crack, that is tU iG 2 t i U aG l (3.106) in which is the total elastic energy and electrical energy stored in the fiber and matrix, which can be expressed in the following form: tU f f f f 0 0 0 m 2 m m 2 m m0 d d d d ( ) 2(1 ) ( ) d d l a L a t z z z z z z z z l l b z rz a U D E r r z D E r r z r r z E E m 2 m m 2 m m ( ) 2(1 ) ( ) d d L b z rz l a r r z E E c (3.107) Then the following energy criterion is introduced: (3.108)i iG G in which is the critical interface debonding energy release rate.icG
- 26. 78 Chapter 3 Fibrous Piezoelectric Composites In Eq. (3.107), is a complex function of the material properties of the con- stituents and geometric factors. Performing the mathematical operation over the debonded and bonded regions for a piezoelectric-epoxy composite system by utilizing a numerical quadrature approach, derived in this study can be obtained as a second-order function of the applied stress for a fiber/matrix system with given debonding length l. tU iG a To illustrate the effect of electromechanical coupling on the debonding behavior of PFCs and to verify the proposed debonding criterion for the piezoelectric fiber push-out problem, a numerical example is considered for two composite systems, namely piezoelectric fiber/epoxy and non-piezoelectric fiber/epoxy. The parameters of the piezoelectric fiber and matrix are given as [8]: 1 1 1 11 33 12 1 1 12 13 55 33 12 3 31 15 33 3 9 2 31 33 0.019 GPa , 0.015 GPa , 0.005 7 GPa , 0.004 5 GPa , 0.039 GPa , 390 10 m/V, 190 10 m/V, 24 10 V m/N, 11.6 10 V m/N, 16.25 10 N/V , f f f f f d d d g g e m m3 GPa, 0.4E The radii of fiber and matrix are given by: The residual fiber clamping stress in the radial direc- tion is –0.1 MPa and 0.065 mm, 3 mm,a b 0.6 mm,l 0q and 2 mm.L 0.8 5/ 400 [8]. It should be pointed out that real piezoelectric fibers have a wide variety of shapes and sizes. In general, the radius a of a piezo- electric fiber is about and the fiber length (More details as to the shape and size of a piezoelectric fiber can be found elsewhere [15,40-42]). In a real single fiber push-out test, in general, the ideal single fiber composite is the one with the value of the matrix radius b being variable, b>>a, and L between 1/2 mm (see[43] for details). m, 200 mmL The geometric configuration and properties of non-piezoelectric fiber matrix and interfaces are the same as those of its counterpart, the piezoelectric fiber, except that the piezoelectric coefficients and dielectric constants are set as zero. To illustrate the effect of electrical loading on stress transfer behavior, Fig. 3.13 presents the distributions of interfacial shear stress as functions of dimensionless axial distance z/L for partially debonded PFCs in the fiber push-out test. In the cal- culation, the debonding length is set to be l = 0.6 mm. The distribution of interfacial shear stress in PFC is similar to that in NPFC [13], in that both show a jump at the point (i.e., the interface between the debonded and bonded regions). It is evi- dent from Fig. 3.13 that there is a larger interface shear stress in the debonded re- gion under an applied negative electrical potential. This is because, for piezoelectric fiber, expansion occurs in the same direction and shrinkage occurs in the transverse direction when the fiber is subjected to an electrical field applied parallel to the po- /l L
- 27. 3.5 Interfacial debonding criterion 79 larization direction. For an applied positive electrical potential, the hoop stress in- duced is in compression while for a negative applied electrical potential, the hoop stress developed is in tension [38]. Therefore, an applied negative electrical loading leads to a larger shear stress in the debonded region than that induced by a positive electrical loading, according to the Coulomb friction law(3.27). Fig. 3.13 Distribution of interfacial shear stress under different electrical loadings for a constant mechanical loading GPa. ( )i z 0.06a The effect of interfacial properties on PFC performance is shown in Fig. 3.14, showing the variation of electrical field as a function of axial distance z/L for several values of the parameters of interfacial properties. It can be seen that the electrical field decreases along with either an increase in the residual compressive stress or an increase in the Coulomb frictional coefficient 0q . These results indicate that for piezoelectric composites, the interfacial properties not only control the stress transfer between fiber and matrix but also have an important influence on the distribution of the electrical field. It should be mentioned that at the transition point from the debonded region to the bonded one there is no jump in electrical field, unlike in the case of interfacial shear stress. This phenomenon is very different from the result obtained in [8], and this difference is mainly attributed to the fact that in our model the expressions for and do not include the term owing to the use of Lamè’s solution [37]. It is also evident from Fig. 3.15 that the results depend largely upon the piezoelectric constant d15. m rr m ,i z To study effect of piezoelectric coefficient on the debonding process, the results of energy release rate are plotted in Fig. 3.15 as a function of debonding length for different piezoelectric coefficients . From this figure we can see that the normalized energy release rate increases along with an increase in the l 15d mG/iG
- 28. 80 Chapter 3 Fibrous Piezoelectric Composites value of . In addition, the energy release rate increases distinctly along with an increase in the value of until it reaches a maximum. This finding implies that the piezoelectric effect has an important influence on the fiber debonding process during fiber push-out. 15d /l L Fig. 3.14 Distribution of electric field in piezoelectric fiber under mechanical loading GPa for different interface property parameters.0.06a Fig. 3.15 Energy release rate vs. under different for a constant me- chanical loading GPa. represents the energy release rate for and . /i mG G mG /l L 15d 0.06a 15 151.0*d d / 0.05l L In Fig. 3.16 the energy release rate vs. electric potential loading is plotted, from which it can be seen that the energy release rate is linearly dependent on the elec-
- 29. 3.6 Micromechanics of fibrous piezoelectric composites 81 trical loading when PFCs are subjected to a constant mechanical loading. The ob- servation above indicates that the total energy release rate can be used as a debond- ing criterion for the piezoelectric fiber push-out test. It should be mentioned that the energy release rate derived in this section is the total energy release rate. Park and Sun [44] obtained the total energy release rate and the mechanical strain rate for an electrically impermeable crack in an infinite piezoelectric medium for the three fracture modes, theoretically and experimentally. They concluded that the total energy release rate could not be used as a fracture criterion because the electrical loading always reduces the total release rate. How- ever, it should be remembered that those results derived from the electrically im- permeable condition on the crack surfaces, a condition not involved in our problem. Fig. 3.16 Energy release rate vs. electrical loading under various mechanical loadings, . represents the energy release rate for electrical loading 0.6 kV./ 0.l L 2 mG 3.6 Micromechanics of fibrous piezoelectric composites In the previous sections of this chapter, stress transfer and interfacial debonding criteria of fibrous piezoelectric composites were described. Determination of the effective material properties of fibrous piezoelectric composites is discussed in this section. It focuses on the developments in [25,26,34]. 3.6.1 Overall elastoelectric properties of FPCs In this subsection some exact results presented in [26,34] for effective properties of a piezoelectric composite consisting of many perfectly-bonded transversely iso-
- 30. 82 Chapter 3 Fibrous Piezoelectric Composites tropic phases of cylindrical shape are briefly summarized. Unlike the format of the constitutive relation (2.2), both Benveniste [34] and Chen [26] employed the five constants of Hill [19] (k, l, m, n, p) in the constitutive relation they studied. For a piezoelectric composite with a fibrous structure charac- terized by the fact that the phase boundaries are surfaces which can be generated by straight line parallel to the x3-axis, the constitutive relations of a class 6mm of the hexagonal system for phase “r” are in the following form: ( ) ( ) 11 11 22 22 33 33 23 23 13 13 12 12 0 0 0 0 0 0 0 0 0 0 0 0 0 0 2 0 0 0 0 0 2 0 0 0 0 0 2 r r r r r r r r r r r r r r r r r r k m k m l k m k m l l l n p p m (3.109) ( ) 31 ( ) ( )31 1( ) 33 2 ( ) 15 3 ( ) 15 0 0 0 0 0 0 0 0 0 0 0 0 0 r r r r r r e e E e E e E e (3.110) T( ) ( ) 31 11 ( ) ( )( ) ( )31 22 111 1( ) 33 ( )33 2 1 ( ) 23 ( )15 3 333 ( ) 13 15 12 0 0 0 0 0 0 0 0 0 0 20 0 0 0 20 0 20 0 0 r r r rr r r r r r r e e D E e D E eD E e 1 2 0 i where k represents the plane strain bulk modulus for lateral dilatation without axial extention, l the associated cross modulus, m the transverse shear modulus, n the modulus for longitudinal uniaxial straining, and p the longitudinal shear modulus. Following the procedure of Chen [26], a representative volume element V of the composite is chosen so that under homogeneous boundary conditions it represents the macroscopic response of the composite. The phase volume fraction cr satisfies c1+c2+ +cN=1, where N is the number of phases in the composite. The volume V is subjected to uniform displacement and electric boundary conditions (3.111)0 ( ) , ( )i ij j iu S x S E x
- 31. 3.6 Micromechanics of fibrous piezoelectric composites 83 where ui and denote the applied elastic displacement and electric potential, and are constant strain and electric field tensors. The overall material properties of the composite are then defined by 0 ij 0 iE 0 T 0 0 ,L e E D e E0 (3.112) where and D stand for the volume average stresses and electric displacements in V. Under the boundary condition (3.111), the relationships between local and global average fields in V are given by 0 0 1 1 1 , , , N N N r r r r r r r r r r r c c cE E D 1 N r c D (3.113) in which cr is the volume fraction of material r, and 1 d r rr V r V V (3.114) In deriving the following formulations for effective material properties, Ben- veniste [34] used two special types of loading condition (3.111): (3.115) 0 111 1 0 2 22 0 3 333 0 3 3 0 0( ) ( ) 0 0 ( ) 0 0 ( ) u S x u S x u S x S E x 2 23 2 (3.116) 0 131 1 0 2 0 0 3 313 23 0 0 1 1 2 2 0 0( ) ( ) 0 0 ( ) 0 ( ) u S x u S x u S x S E x E x Under the loading condition (3.115), the solution can be assumed in the form (3.117) ( ) ( ) ( ) ( ) 1 1 1 2 2 2 1 2 ( ) 0 ( ) 0 3 33 3 3 3 ( , ), ( , ), , r r r r r r u u x x u u x x u x E x The resulting stresses, electric displacements, equilibrium equations, and conti- nuity conditions are
- 32. 84 Chapter 3 Fibrous Piezoelectric Composites (3.118) ( ) ( ) ( ) 0 ( ) 0 11 1,1 2,2 33 31 3 ( ) ( ) ( ) 0 ( ) 0 22 1,1 2,2 33 31 3 ( ) ( ) ( ) 0 ( ) 0 33 1,1 2,2 33 33 3 ( ) ( ) ( ) 12 1,2 2,1 ( ) ( ) ( ) 3 31 1,1 ( ) ( ) ( ) ( ) ( ) , ( ), ( r r r r r r r r r r r r r r r r r r r r r r r r r r r r r k m u k m u l e E k m u k m u l e E l u u n e E m u u D e u ( ) ( ) 0 ( ) 0 2,2 31 33 33 3 ( ) ( ) ( ) ( ) 23 13 1 2 ) , 0 r r r r r r r u e E D D , , r r 0, 0 (on )rs 2x r (3.119) ( ) ( ) ( ) ( ) 1,11 2,21 1,22 2,12 ( ) ( ) ( ) ( ) 1,12 2,22 1,21 2,11 ( ) ( ) ( ) ( ) ( ) ( ) r r r r r r r r r r r r r r r r r r k m u k m u m u u k m u k m u m u u (3.120) ( ) ( ) ( ) ( ) 1 1 2 2 ( ) ( ) ( ) ( ) 11 1 12 2 11 1 12 2 ( ) ( ) ( ) ( ) 21 1 22 2 21 1 22 2 , , , r s r s r r s s r r s s u u u u n n n n n n n n where n = (n1, n2,0) denotes the normal to the interface rs which is the interfaces between phase r and phase s. For the loading condition (3.116), the corresponding solutions can be assumed in the form (3.121) ( ) 0 ( ) 0 1 13 3 2 23 3 ( ) ( ) 0 0 ( ) ( ) 3 1 2 13 1 23 2 1 , , ( , ) , ( , ) r r r r r r u x u x u x x x x x The stresses and electric displacements induced by the fields (3.121) are ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) 23 ,2 15 ,2 13 ,1 15 ,1 ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) 1 15 ,1 11 ,1 2 15 ,2 11 ,2 , , , r r r r r r r r r r r r r r r r r r r p e p e D e D e (3.122) whereas the equilibrium equation (3.119) becomes (3.123)2 ( ) ( ) ( ) ( ) 2 ( ) ( ) ( ) 15 15 110, 0r r r r r r r rp e e in which the functions ( ) ( ) andr r can be obtained by solving (3.123) under the boundary conditions (3.116) and the following continuity conditions at the inter- faces rs: (3.124) ( ) ( ) ( ) ( ) 1 1 2 2 ( ) ( ) ( ) ( ) 11 1 12 2 11 1 12 2 ( ) ( ) ( ) ( ) 21 1 22 2 21 1 22 2 , , , r s r s r r s s r r s s u u u u n n n n n n n n (on )rs
- 33. 3.6 Micromechanics of fibrous piezoelectric composites 85 3.6.1.1 Effective properties of two-phase composites (1) Effective constants of k, l, n, e31, e33, and 33. To determine k, assume and in Eq.0 11 22 0 0 0 33 3 0E (3.115). Then, Eqs. (3.117)-(3.120) show that this turns out to be a purely mechanical problem and k can be expressed as [34] f m m f m m m 1 c k k c k k k m (3.125) where the subscripts “m” and “f ” represent the related variables which are associ- ated with matrix phase and fiber phase. The formulae for the remaining five con- stants can be obtained by making use of the universal connections between these moduli as recently derived by Schulgasser [22]: (m) (f) m 31 f 31 31f m m m f f (m) (f) f m m m f f m 33 f 33 33 (m) (f) 31 m 31 f 31f m m m f f (f) (m) (m) (f) (m) (f) 31 31 31 31 m 33 f 33 33 m 33 f 33 33 , c e c e ek k k k c l c l l l l l l c n c n n c e c e e e c e c ek k k k c l c l l e e e e c e c e e c c (3.126) It is noted that only five of the six relations in Eq. (3.126) are independent. Once k is known from Eq. (3.125), the effective material constants l, n, e31, e33, and 33 can be determined from Eq. (3.126). (2) Effective constants of e15, p, and 11. The determination of these three constants involves the application of boundary condition (3.116) and the use of Eqs. (3.121)-(3.124). For simplicity, rewrite the constitutive equation (3.122) in matrix form (3.127) ( ) ( ) ( )( ) 15 ( ) ( ) 15 11 r rr r rr r p e e L D r The real symmetric matrix Lr can be diagonalized by means of the transformation (3.128)* T ( m,f)r r rL WL W where W may be complex, and is diagonal.* rL Now define (3.129) ( ) ( )( ) ( )* * 1T * * , r rr r W W DD so that there is
- 34. 86 Chapter 3 Fibrous Piezoelectric Composites (3.130) ( ) ( )* * * * * * , 0, 0 r r rL D D * T Therefore, in terms of the new field quantities, the original coupled problem is reduced to two uncoupled problems. The transformed effective tensor L* is also diagonal. That is, (3.131)* L WLW with (3.132) * 15* * 15 1111 0 , 0 p ep e L L The above procedures imply that use can be made of known results in the uncou- pled system to transform them to the coupled system. The composite cylinder re- sults for p* and are given by [34]* 11 * * * * m m f f m * * m f f m * * m 11 11 f* * m f 11 11 m * * 11 f 11 mm f (1 ) , (1 ) (1 ) (1 ) c p p c p p p c p c c c c c (3.133) Equation (3.133) can be written in matrix form as 1** m ** 1111 m 00 0 0 000 pp H F 0 J G (3.134) where * * * * m f f m 11 f 11 mm * * * * m m f f m 11 11 fm f (1 ) , (1 ) , (1 ), (1 ) f H p c p c J c c F c p p c G c c (3.135) To transform the L* into L, multiply each side of Eq. (3.134) by W–1 and WT–1 respectively, and after some mathematical manipulation, we obtain (3.136)1 m f m m f m m f f[(1 ) ] [ (1 ) ]c c c cL L L L L L Equation (3.136) gives the effective constants p, e15, 11 of two-phase FPCs. 3.6.1.2 Effective properties of FPC with equal transverse shear modulus Consider a multiphase FPC with the same transverse shear modulus for all phases and with transversely isotropic constituents described by the constitutive
- 35. 3.6 Micromechanics of fibrous piezoelectric composites 87 laws (3.109) and (3.110). The method of derivation follows closely the analysis of Hill [19] for the uncoupled mechanical case. Let the composite be subjected to the loading condition (3.115), resulting the following fields: ( ) ( ) ( ) ( ) ( ) 0 ( ) 01 2 1 2 1 2 3 33 3 1 2 ( , ) ( , ) , , , r r r r rf x x f x x u u u x x x 3 3 r E x , , r r (3.137) where f is an unknown function to be determined from the governing equation and boundary conditions. Substituting Eq. (3.137) into Eqs. (3.109) and (3.110) yields [26] (3.138) ( ) ( ) ( ) 0 ( ) 0 11 ,11 ,22 33 31 3 ( ) ( ) ( ) 0 ( ) 0 22 ,11 ,22 33 31 3 ( ) ( ) ( ) 0 ( ) 0 33 ,11 ,22 33 33 3 ( ) ( ) 12 ,12 ( ) ( ) ( ) ( ) ( 3 31 ,11 ,22 31 ( ) ( ) ( ) ( ) ( ) , 2 , ( ) r r r r r r r r r r r r r r r r r r r r r r r r r k m f k m f l e E k m f k m f l e E l f f n e E mf D e f f e ) 0 ( ) 0 33 33 3 ( ) ( ) ( ) ( ) 23 13 1 2 , 0 r r r r r E D D Benveniste [34] indicated that Eq. (3.119) are identically satisfied by requiring 2 ( ) ( ) ( ) 11 22 r r r rf e (3.139) where er conforms with the uniform phase dilatations. It can be proved that the in- terface conditions of surface traction (3.124) are satisfied if [34] (3.140)0 ( ) 0 0 ( ) 33 31 3 33 31 3( ) ( )s s s s r r rk m e l e E k m e l e E0r 0 E For any two phases r and s, Eq. (3.140) together with the condition (3.141)0 0 11 22 1 N r r r c e enable us to determine the constants er. After a series of mathematical manipula- tions, Benveniste [34] obtained the expression for er as (3.142)0 0 0 11 22 33 3( )r r r re where ( ) 31 ( ) 1 31 1 1 1 1 , , sN s r ss r r rN N r r rs s s ss s c e k m c e k m k m k mc c k m k m 1
- 36. 88 Chapter 3 Fibrous Piezoelectric Composites 1 1 1 N s s ss r r r N r rs ss c l k m c l k m k mc k m (3.143) Then, the average fields used to determine the effective constants are obtained as 0 0 0 11 11 22 33 31 3( ) ( )k m k m l e E0 ( ) ( ) 0 ( ) 0 11 22 33 31 3 1 ( ) ( ) N r r r r r r r r r r c k m c k m c l c e Er (3.144) 0 0 0 22 11 22 33 31 3( ) ( )k m k m l e E0 ( ) ( ) 0 ( ) 0 11 22 33 31 3 1 ( ) ( ) N r r r r r r r r r r c k m c k m c l c e Er (3.145) 0 0 0 33 11 22 33 33 3( )l n 0 e E ( ) ( ) 0 ( ) 0 11 22 33 33 3 1 ( ) N r r r r r r r r r c l c n c e E (3.146) 0 12 12 12 1 2 N r r r m c m ( ) (3.147) 0 0 0 3 31 11 22 33 33 33( )D e e E0 3 ( ) ( ) ( ) ( ) 0 ( ) 0 33 11 22 33 33 33 3 1 ( ) N r r r r r r r r c e c e c Er (3.148) Making use of Eqs. (3.144)-(3.148), Benveniste [34] obtained the following formu- lations for predicting effective material constants k, l, n, e31, e33, and 33: ( ) 31 1 1 31 1 1 , , 1 1 sN N N rr r r r r rr r r N N N r r r rr r r c ec k c l k m k m k m k l e c c k m k m k m r r r c (3.149) 2 1 1 1 1 1 N r r N N N rr r r r r r r N r rr r rr rr c n k mc n c n n c n k m k mc k m (3.150)
- 37. 3.6 Micromechanics of fibrous piezoelectric composites 89 ( ) 33 2( )( ) 33( ) 33 1 33 33 1 1 1 1 rN r rrN N N rr rr r r N r rr r rr rr c e c ek mc e e c e k m k mc k m (3.151) ( ) 33 2( )( ) 33( ) 33 1 33 33 1 1 1 1 rN r rrN N N rr rr r r N r rr r rr rr c ck mc c k m k mc k m (3.152) 3.6.2 Extension to include magnetic and thermal effects In the last subsection, a formulation for effective elastoelectric material constants of FPCs was presented. Extension of these results to include piezomagnetic and thermal effects is presented in this subsection. It is a brief review of the development in [25]. To obtain formulations for calculating effective constants of thermo-magneto- electro-elastic materials, Benveniste [25] considered a transversely isotropic, two-phase composite with a fibrous structure. The constitutive law is given by (3.153) ( ) ( ) ( ) T( ) ( ) T( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) , , r r r r r r r r r r r r r r r r r r r r r r r r r r r c e E e H D e E H B e E H where denote, respectively, magnetic fluxes, magnetic field intensity, and temperature change in rth phase; Elastic properties is a 6 6 elastic constant matrix defined in Eq. (3.109); are piezoelectric and dielectric constants defined in Eq. (3.110). are thermal stress, pyroelectric, and pyromagnetic vectors. are piezomagnetic, magnetoelectric coupling coefficient, and magnetic permeabilities matrices. These six matrices are defined by ( ) ( ) ( ) , , andr r B H r r r , ( )r c ( ) ( ) andr e ( ) ( ) , , andr r ( ) ( ) , , andr r ( ) ( ) r e (3.154) T( ) ( ) ( ) ( ) T T L T( ) ( ) L T( ) ( ) 3 0 0 0 , 0 0 , 0 0 r r r r r r r r ( ) 15 ( ) 15 31 31 33 0 0 0 0 0 0 0 0 0 0 0 0 0 r r e e e e e e
- 38. 90 Chapter 3 Fibrous Piezoelectric Composites (3.155) ( ) ( ) 11 11 ( ) ( ) 11 11 33 33 0 0 0 0 0 0 , 0 0 0 0 0 0 r r r r where T and L are transverse and longitudinal thermal stress coefficients, L is the longitudinal pyroelectric constant. Benveniste [25] then considered the following two sets of loading conditions: The first set of loading conditions consists of Eq. (3.115) and 0 3 3 0( ) , ( )S H x S , (3.156) where is magnetic potential. The second set of loading conditions is defined by Eq. (3.116) and (3.157)0 0 1 1 2 2( )S H x H x together with the steady state equilibrium equations (3.158), ,0, 0, 0ij j i i i iD B Keeping this mind, he proved that there exists a specific choice of , denoted by , so that the strains, electric and magnetic fields are uniform throughout the composite: 0 0 0 0( , , , )E H 0 ˆ ˆˆ( , , , )E H ( ) ( ) ( ) 0 ˆ ˆˆ, , ,r r r E E E H H H (3.159) and the possible sets of resulting in uniform fields are given by0 ˆ ˆˆ( , , , )E H 1 2 3 1 2 3 43 3 3 33 4 5 6 1 2 1 2 ˆ 01 0 0 ˆ 01 0 0 ˆ 1 ,1 ˆ 00 ˆ 0 0 0 ˆ ˆ ˆ ˆˆ ˆ ˆ 0 r r E s tH E E H H 03 0 (3.160) where ( 1- 4)i i are arbitrary constants and (3.161) 3 1 2 1 2 (1) (2) 3 1 2 31 31 (1) (2) 3 1 2 31 31 (1) (2) 3 T T 1 2( )/( ), ( ) /( ), ( ) /( ), ( ) /( r k k l l s l l e e t l l e e r l 2 )l where subscripts “1” and “2” represent the variables associated with matrix and fiber materials. The uniform fields generated from Eq. (3.160) allow the derivation of exact connections between some of the effective properties. The effective con-
- 39. 3.6 Micromechanics of fibrous piezoelectric composites 91 stants c, e, q, , , , , , are defined by T T 0 2 ( ) ( ) T( ) ( ) T( ) ( ) ( ) 0 1 0 2 ( ) ( ) ( ) ( ) ( ) ( ) ( ) 0 1 ( ) ( ) 0 2 ( ) ( ) ( ) ( ) ( ) ( ) ( ) 0 1 [ ] [ ] [ ] r r r r r r r r r r r r r r r r r r r r r r r r r r r r r c c c c e E e H c e E e H D e E H e E H B e E H e E H , , (3.162) Substituting Eqs. (3.159) and (3.160) into Eq. (3.162) and equating the coeffi- cients , 1- 4i i yield a set of exact connections between the effective properties as follows [24,25]: 2 2 2 ( ) 31 31 1 1 1 1 2 2 2 ( ) 1 2 33 33 1 1 1 r r r r r r r r r r r r r r r r r r k c k l c l e c e k k l l l c l n c n e c e 2 (3.163) 2 2 2 ( ) ( ) ( ) 31 31 33 33 33 33 (1) (2) 31 311 1 1 2 2 2 ( ) 1 2 33 33 1 1 1 r r r r r r r r r r r r r r r r r r e c e e c e c e e l l l c l n c n e c e (3.164) 2 2 2 ( ) 31 31 1 1 1 1 2 2 2 (1) ( ) ( ) ( ) 31 31 31 31 33 33 33 33 1 1 1 r r r r r r r r r r r r r r r r r r k c k l c l e c e e e e c e e c e c 2 (2) (3.165) 2 2 2 ( ) ( ) ( ) 31 31 33 33 33 33 (1) (2) 31 311 1 1 2 2 2 ( ) 1 2 33 33 1 1 1 r r r r r r r r r r r r r r r r r r e c e e c e c e e l l l c l n c n e c e (3.166) 2 ( ) 33 33 1 1 2 (1 ( ) 31 31 33 33 1 r r r r r r e c e l l e e c 2 ) (2) (3.167)
- 40. 92 Chapter 3 Fibrous Piezoelectric Composites 2 2 ( ) 1 2 3 T 1 1 r r r r r r c l l r c L (3.168) 2 2 ( ) 3 3 1 1 r r r r r r c n n r c (3.169) 2 2 ( ) ( ) 3 33 33 3 1 1 r r r r c e e r c L r r (3.170) (3.171) 2 2 ( ) ( ) 3 33 33 3 1 1 r r r r c e q r c 3 r r 2x c On the whole, there are nine independent connections between the ten effective parameters k, l, n, e33, e31, 33, 33, 33, so that knowledge of one of them allows the determination of the rest. In [25], it was proved that the parameter k can be determined by Eq. (3.125). Having obtained the value of k, the moduli l, n, e33, e31, 33, 33, 33 can thus be fully determined from Eqs. (3.163)-(3.167) above. 31 33, ,e e 31 33, ,e e The remaining six effective constants ( p, e15, 33, 33, 33 ) can be deter- mined using the procedure described in [25]. Consider the loading type defined by Eqs. (3.116) and (3.157). The solution to this loading type can be represented by 15 ,e (3.172) ( ) 0 ( ) 0 ( ) ( ) 0 0 1 13 3 2 23 3 3 1 2 13 1 23 ( ) ( ) ( ) ( ) 1 2 1 2 , , ( , ) , ( , ), ( , ) r r r r r r r r u x u x u x x x x x x x Benveniste [25] then cast the constitutive laws of the constituents in matrix form as (3.173) ( )( ) ( ) 15 15 15 11 11 15 11 11 ( 1,2, ) rr r p e e e r e D B where the subscript “c” refers to the effective law, and the following definitions are used: 13 23 1 2 1 2 ,1 ,2 ,1 ,2 ,1 ,2 , , , , , D D B BD B (3.174) Similar to the procedure described in Subsection 3.6.1.1, define the 3 3 matrices Lr representing the material matrix in Eq. (3.173):
- 41. 3.6 Micromechanics of fibrous piezoelectric composites 93 (3.175) ( ) 15 15 15 11 11 15 11 11 ( 1,2, ) r r p e e e e L r c c 1 c Lr can then be converted to a diagonal matrix using a matrix W:* rL (3.176)* T ( 1,2, )r r rL WL W The implication of this result is the existence of the following constraint relation between the components of the effective matrix Lc: (3.177)1 1 2 2 1cL L L L L L It can be shown that the resulting matrix on the left hand side of Eq. (3.177) is antisymmetric, so that this equation provides three connections between the six effective components to be determined. To find the remaining three connections, consider the uncoupled elastic, electric, and magnetic behavior of the composite and denote the longitudinal shear modulus, transverse dielectric, and magnetic per- meability coefficients by In the framework of the composite cylinder assemblage model [45], Benveniste [25] obtained the following expres- sions of * * * 11 11, , and .p * :* * 11 11, , andp * * * * 1 1 2 2 1 * * 2 1 1 2 (1 ) ( , , ) (1 ) c f c f f f f p c f c f 11 11 c 2 2 (3.178) He then defined the matrices * :rL (3.179) * * * 11 * 11 0 0 0 ( ) 0 ( 1,2, ) 0 0 ( ) r r r r p rL and cast Eq. (3.178) in the form (3.180)* * * * 1 * * 1 2 1 2 2 2 1 2[(1 ) (1 ) ] [(1 ) (1 ) ]c c c c cL L L L L L Making use of Eq. (3.176), it can be proved that the effective moduli of the piezo- magnetoelectric composite is given by (3.181)1 1 2 1 2 2 2 1 2[(1 ) (1 ) ] [(1 ) (1 ) ]c c c c cL L L L L L where L1, L2, and Lc are defined by Eq. (3.175).
- 42. 94 Chapter 3 Fibrous Piezoelectric Composites 3.7 Solution of composite with elliptic fiber In this section, the thermoelectroelastic solutions presented in [35] for thermal loading applied inside and outside an elliptic piezoelectric fiber in an infinite piezo- electric matrix are presented. By combining the method of Stroh’s formalism, the technique of conformal mapping, the concept of perturbation and the method of analytical continuation, a general analytical thermoelectroelastic solution is ob- tained for an elliptic piezoelectric cylindrical fiber embedded in an infinite piezo- electric matrix subjected to thermal loading. The loading may be a point heat source, temperature discontinuity, or a uniform remote heat flow. Special cases when the fiber becomes rigid or a hole are also investigated. 3.7.1 Conformal mapping Consider an elliptic piezoelectric fiber embedded in an infinite matrix. The contour of their interface is represented by 1 2cos , sinx a x b (3.182) where is a real parameter and are the principal radii of the elliptic interface. It will be more convenient to transform the ellipse to a circle before solv- ing the problem. For this, consider the mapping 0a b 1 1 2k k k k kz a a (3.183) where (3.184)1 2( )/ 2, ( ) / 2k k k ka a ip b a a ip b Equation (3.183) will map the region outside the elliptic fiber onto the exterior of a unit circle in the k-plane. Further, the transformation (3.183) is single valued and conformal outside the ellipse, since the roots of equation (3.185)2 1 2d / d 0k k k k kz a a are located inside the unit circle 1k . In fact, the roots are 0 2 1/k ka a k ,ki km e where (mk)1/2 <1 [46]. However, the mapping (3.183) is not single valued inside the ellipse because the roots of Eq. (3.185) are located inside the unit circle. To bypass this problem, the mapping of 2 (see Fig. 3.17) is done by ex- cluding a slit 0, which represents a circle of radius km in the k-plane, from the ellipse [47]. In this case the function (3.183) will transform and 0 into a ring of outer and inner circles with radii andout 1r in kr m , respectively. Moreover,
- 43. 3.7 Solution of composite with elliptic fiber 95 anywhere inside the ellipse and on the slit 0 a function f ( k) must satisfy the following condition: 2 [ ( )] [ / (ki k kf m f m e )] (3.186) to ensure that the field is single valued [47], where stands for a point located on the unit circle in the k-plane, and is a polar angle. ( ) i e Fig. 3.17 Geometry of an elliptic fiber in a matrix. 3.7.2 Solutions for thermal loading applied outside an elliptic fiber Consider an elliptic fiber embedded in an infinite piezoelectric matrix subjected to thermal loading located at the point (x10, x20) which is outside the fiber. If the fiber and matrix are assumed to be perfectly bonded along the interface, the temperature, heat flow (hn), elastic displacements, electric potential, stress and electric displace- ment (tn) across the interface should be continuous, i.e., (along the interface) (3.187)1 2 1 2 1 2 1, = , = , =T T U U 2 ,s Here the following equations are used: (3.188), ,n s nh t where n is the normal direction of the interface, s is the arc length measured along the elliptic boundary, and tn is the surface traction-charge vector. Here and in the following, the subscripts “1” and “2” (or superscripts (1) and (2)) denote the quanti- ties associated with matrix and fiber, respectively. 3.7.2.1 General solution for thermal fields Based on the conformal mapping described above and the concept of perturbation
- 44. 96 Chapter 3 Fibrous Piezoelectric Composites given by Stagni [48], the general solution for temperature and heat-flow function can be assumed in the form (1) (1) (1) (1) 1 0 0 1 1 (1) (1) (1) (1) 1 1 0 1 0 1 1 1 1 ( ) ( ) ( ) ( ), ( ) ( ) ( ) ( ) t t t t t t t T f f f f ik f ik f ik f ik f t (1) )( 1t (3.189) (2) (2) 2 2 2 (2) (2) 2 2 2 2 2 ( ) ( ), ( ) ( t t t t T f f ik f ik f ) (2) 2( )t 2 (3.190) Here, f0 can be chosen to represent the solutions associated with the unperturbed thermal field, which is holomorphic in the entire domain except for some singular points such as the point at which a point heat source is applied, and f1 and f2 are the functions corresponding to the perturbed field of matrix and fiber, respectively. They are holomorphic in the regions , respectively. In the t-plane, is the region outside the unit circle and is the region of the annular ring be- tween the unit circle and the circle of radius 1 and 2 1 tm . For a given loading condition, the function f0 can be obtained easily since it is related to the solution of homogeneous media. When an infinite space is subjected to a line heat source h* and a line temperature discontinuity ,both located at (x10, x20), the function f0 can be chosen in the form ˆT (3.191)(1) (1) (1) 0 0( ) ln(t tf q 0 )t twhere (1) (1) 0andt are related to the complex arguments through the following transformation functions: (1) (1) 0 1and (t tz z 0x *(1) 1p x20 ) (1) (1)2 2 *(1)2 2 1(1) *(1) 1 t t t z z a p b a ip b , (1) (1)2 2 *(1)2 2 0 0 1(1) 0 *(1) 1 t t t z z a p b a ip b (3.192) and q0 is given in the form [36] (3.193)* 0 ˆ / 4 / 4q T i h k When the thermal load is uniform remote heat flow , the function f0 may be expressed by 10 20( , )h hh (1) * (1) 0 0( )tf q t (3.194) The infinite condition provides
- 45. 3.7 Solution of composite with elliptic fiber 97 * *(1) *(1) 0 1 10 1 1 1 ( )( / 4 q a ibp h p h ik 20 ) (3.195) As for the function f2, noting that it is holomorphic in the annular ring, it can be represented by Laurent’s series (2) (2) 2 ( ) j t j j f c t (3.196) whose coefficients can be related by means of Eq. (3.186) in the following manner: *(2) * * 1 *(2) 1 , j j j j j a ibp c c a ibp (3.197) Inserting Eqs. (3.191) and (3.196) into Eqs. (3.189) and (3.190), and later into Eqs. (3.187)1,2, yields * * 1 0 1 0 1 1 ( ) ( ) [ ] [ ] ( ) ( )j j j j j j j j j j f f c c c c f f (3.198) *2 0 1 1 1 ( ) ( ) [ ] j j j j j k f f c c k *2 0 1 1 1 [ ] ( )j j j j j k c c f f k ( ) (3.199) One of the important properties of holomorphic functions used in the method of analytic continuation is that if the function f( ) is holomorphic in 1 (or then 0 2 ), (1/ )f is holomorphic in (or 1), 0 denoting the region inside the circle of radius 0 2 tm . Hence, put * 1 0 1 1 * 1 0 0 1 ( ) (1/ ) [ ] ( ) ( ) (1/ ) ( ) [ ] ( ) j j j j j j j j j j f f c c f f c c 2 (3.200) where the function ( ) is holomorphic and single valued in the whole plane. By Liouville’s theorem, we have ( )= constant. However, constant function f does not produce stress and electric displacement (SED), which may be neglected. Thus, by letting ( )=0, we have
- 46. 98 Chapter 3 Fibrous Piezoelectric Composites * 1 0 1 1 * 1 0 0 1 [ ] ( ) (1/ ) ( ) [ ] (1/ ) ( ) ( ) j j j j j j j j j j c c f f c c f f 2 (3.201) It should be mentioned that the subscripts “1” and “2” (or superscripts (1) and (2)) are omitted in Eqs. (3.200) and (3.201). To further simplify subsequent writing, we shall omit them again in the related expressions when the distinction is unne- cessary. As in Eq. (3.201), it can be determined from Eq. (3.199) that *2 1 0 1 1 1 *2 1 0 0 1 1 [ ] ( ) (1/ ) ( ) [ ] (1/ ) ( ) ( ) j j j j j j j j j j k c c f f k k c c f f k 2 (3.202) The Eqs. (3.201)2 and (3.202)2 provide * 0 2 1 2 1 1 1 ( ) [(1 / ) (1 / ) ] 2 j j j j f k k c k k jc (3.203) With the use of the series representation ( ) 0 0 1 1 (0) ( )1 ( ) , d ! 2 k k k k kC k f f0 x f x e x e k i x x (3.204) the function f0( ) given in Eq. (3.191) (or (3.194)) can be expressed as (1) 0 0 0 1 ( ) , j j t j j j q f e e j * 1 0(or )j je q (3.205) where ij=1, when i=j; ij=0, when i j. By comparing the coefficients of corresponding terms in Eqs. (3.203) and (3.205), we obtain 1 0 0 0( / ) ( / ) ( 1, 2, , )j j j j j jc G G G G e G e G j (3.206) where .* 0 2 1 2 1(1 / ) / 2, (1 / ) / 2j jG k k G k k With the solution obtained for ck, the functions f1, 1, and 2g g can be further written as * (1) (1) 1 (1) 1 0 1 ( ) lnj j j j t t t j f c c q 0 (3.207)
- 47. 3.7 Solution of composite with elliptic fiber 99 (1) (1) (1) (1) 1 (1) * (1) 1 0 0 0 0 1 ( ) ln( ) ln( ) j t t t t t j j j j g q q c c t (3.208) (2) (2) * (2) 2 1 ( ) j j t j t j t j g c (3.209) Equations (3.208) and (3.209) are the general thermal solutions for the case of line heat source and temperature discontinuity. If the load is uniform remote heat flow, the general solutions can be obtained similarly. They are (1) * (1) * (1) 1 * (1) 1 1 0 0 1 1 1( ) ( )t t t tg q q c c ) i g (3.210) (3.211)(2) (2) * (2) 1 2 1 1( ) (t t tg c 3.7.2.2 General solution for electroelastic fields The particular piezoelectric solution induced by a thermal load can be written as [35,36] (i=1,2) (3.212)( ) ( ) 2Re[ ( )], 2Re[ ( )]i ip i i t ip i i tgU c d where subscript “p” refers to a particular solution. The function g(zt) in Eq. (3.212) can be obtained by integrating Eqs. (3.208) and (3.209) (or (3.210) and (3.211)) with respect to zt, which yields (1) (1) (1) (1) (1) 1 (1) (1) (1) (1) 1 1 0 1 0 0 2 0 2 0 2( ) [ ( , ) ( , )] [ ( ,t t t t t tg a q F q F a q F 0 )t (1) 1 (1) * (1) (1) (1) 0 1 0 1 1 1 1 1 1 ( , )] ( ) ln j t t t j t j q F c c a G (3.213) (2) (1) (2) 2 2 3 1 ( ) j j t j t j t j g G G (3.214) for Eqs. (3.208) and (3.209), or (1) * (1) (1)2 (1) (1) 1 0 1 2( ) ( / 2 lnt tg q a a )t * * (1) (1) (1) (1) 2 0 1 1 1 1 2( )( ln t tq c c a a / 2) 2 (3.215) (3.216)(2) (2) (2)2 (2) * (2) 2 2 1 1 2 1( ) ( )/t t tg c a a for Eqs. (3.210) and (3.211), where 1 0 0 0( , ) ( )[ln( ) 1],t t t t t tF 1 1 1 2 0 0 0 0 ( ) *( ) ( ) *( ) 1 1 2 1 ( , ) ( )ln( ) ln , ( ) / 2, ( )/ 2, ( 1, 2) t t t t t t t t k k k k F a a ip b a a ip b k
- 48. 100 Chapter 3 Fibrous Piezoelectric Composites * (1) (1) * 1 1 1 1 1 2 1 1 1 1 (2) (2) 2 1 1 1 2 1 (2) * (2) * 3 1 1 1 2 1 1 1 [( ) ( ) ]/ , ( ) / , ( ) / j j j j j j j j j j j j j j j j j j G c c a a c c s j G a c s a c j G a c a c s j (3.217) and 1 for , 0 forij ijs i j s i j . The particular solution (3.212) does not generally satisfy the condition (3.187)3,4 along the interface. We therefore need to find a corrective isothermal solution for a given problem so that when it is superposed on the particular thermoelectroelastic solution the interface condition (3.187)3,4 will be satisfied. Owing to the fact that f( m) and g( t) have the same rule affecting the SED in the general solution of a thermoelectroelastic problem [35] 1 ,2 2 ,1 1 ,2 2 ,1 ( ) ( ), ( ) ( ), , , ( ) ( ) ( ) ( ), ( ) ( ) ( ) ( ), , t t t t t t t t T g z g z ikg z ik g z h h f z g z f z g z f z g z f z g z U A q c A q c B q d B q d (3.218) with (3.219)* 1 1tz x p x2 possible function forms come from the partition of g( t). They are ( ) ( ) ( ) ( ) ( ) ( ) 1 0 1 0 0 2 0 ( ) 1 ( ) ( ) 1 ( ) 0 1 0 0 2 0 ( ) ( ) ( ) ( ) ( ) ( ) ( ) 2 0 1 0 0 2 0 ( ) [ ( , ) ( , ) ( , ) ( , )]/ 2, ( ) [ ( , ) ( , ) j j j j j j m m m t m t j j j j m t m t j j j j j j j m m m m t m t f a q F q F q F q F f ip b q F q F q 0 ( ) 1 ( ) ( ) 1 ( ) 1 0 0 2 0( , ) ( , )]/j j j j m t m tF q F 2 ( j=1,2) (3.220) ( ) ( ) ( ) ( ) 3 1( ) lnj j j m m m mf a j ( j=1,2) (3.221) ( ) ( ) ( ) ( ) ( ) ( ) ( ) ( ) 4 5 1 1 ( ) , ( )j j j k j j j j k j k k k k f r f s ( j=1,2) (3.222) where ( )j kf are four component vectors, and ( ) ( ) andj j kr sk are constant vectors with four components to be determined. It should be pointed out that the vector ( )j ks is not the same as the symbol sij given in Eq. (3.217).
- 49. 3.7 Solution of composite with elliptic fiber 101 The Green’s functions for the electroelastic fields can thus be chosen as 3 5 ( ) ( ) ( ) ( ) ( ) ( ) 1 4 2Re ( ) ( ) ( )j j j j j j j j k k j k j j k k f gU A q A f c t (3.223) 3 5 ( ) ( ) ( ) ( ) ( ) ( ) 1 4 2Re ( ) ( ) ( )j j j j j j j j k k j k j j k k f gB q B f d t (3.224) The above two expressions, together with the interface condition (3.187)3,4, pro- vide (1) 1 1 1 1 2 1 2 1(q X A c B d ) (3.225) (2) 1 1 1 2 1 1 1(q X B d A c1) (3.226) (1) *(1) 1 (1) 2 1 1 1pq P q (3.227) (2) (*1) 1 (2) 2 1 2 1pq P q (3.228) 1(1) (1) (1) * (1) 3 1 1 1 1 1( )a a c cq 1q (3.229) 1(2) (2) (1) * (2) 3 1 1 1 1 1 1( )a a c cq q (3.230) (1) (1) (2) (2) 1 5 1 4 2 5 2 4 1 1 2 2 2 3 1 ( ) ( ) ( ) ( ) ( ) j j j j j G G GA f A f A f A f c c c (2) (2) (1) (1) 2 4 2 5 1 4 1 5 1 1 2 2 2 3 1 = ( ) ( ) ( ) ( ) ( ) j j j j j G G GA f A f A f A f c c c (3.231) (1) (1) (2) (2) 1 5 1 4 2 5 2 4 1 1 2 2 2 3 1 ( ) ( ) ( ) ( ) ( ) j j j j j G G GB f B f B f B f d d d (2) (2) (1) (1) 2 4 2 5 1 4 1 5 1 1 2 2 2 3 1 = ( ) ( ) ( ) ( ) ( ) j j j j j G G GB f B f B f B f d d d 1 (3.232) where (3.233)1 1 1 1 1 1 2 1 2 1 2 1 2 1 2( ) , ( )X A A B B X A A B B Therefore, by Liouville’s theorem, Eqs. (3.231) and (3.232) yield
- 50. 102 Chapter 3 Fibrous Piezoelectric Composites (2) (2) 2 5 2 4 1 1 2 2 2 3 1 ( ) ( ) ( ) j j j j j G G GA f A f c c c (1) (1) 1 5 1 4( ) ( )A f A f (3.234) (2) (2) 2 4 2 5 1 1 2 2 2 3 1 ( ) ( ) ( ) j j j j j G G GA f A f c c c (1) (1) 1 4 1 5( ) ( )A f A f (3.235) (2) (2) 2 5 2 4 1 1 2 2 2 3 1 ( ) ( ) ( ) j j j j j G G GB f B f d d d (1) (1) 1 5 1 4( ) ( )B f B f (3.236) (2) (2) 2 4 2 5 1 1 2 2 2 3 1 ( ) ( ) ( ) j j j j j G G GB f B f d d d (1) (1) 1 4 1 5( ) ( )B f B f (3.237) The above four equations are not completely independent. For example, Eqs. (3.234) and (3.236) can be obtained from Eqs. (3.235) and (3.237). Thus only two of the equations are independent. However, there are four sets of constant vectors, i.e., , to be determined. We need two more equations to make the solution unique. Through use of the relation (3.186) and Eqs. (3.223) and (3.224), the unknown vectors ( ) ( ) and ( 1,2)j j k k jr s (2) (2) andj jr s appearing in can be determined as follows: (2) (2) 4 andf f5 (2) 1 (2) 1 (2) 1 1 2 2 2 2 2 2( ) 3[ (j j j Gr A A B B A c j (2) 1 (2) 2 2 2 2 3 2 2) ( )] ( 1, , )j j j j jG G G jc B d d (3.238) (2) 1 (2) (2) 2 2 2 2 2[ ( ) 3 ]j j j jG Gs B B r d d j )( 1 (3.239), ,j where ( ) ( ) ( ) ji i j i a ibp a ibp . Once the constant vectors (2) (2) andj jr s are obtained, the unknown vectors (1) (1) andj jr s given in can be determined from Eqs. (3.234) and (3.236) (or (3.235) and (3.237)). They are (1) 4 andf (1) 5f (1) T (2) (2) 1 2 1 2 1 2 2[( ) ( )j j jir A M M A r M M A s 1 1 1 2 2 2 3 1 1 2 2 2 3( ) ( )]j j j j jG G G i G G GM c c c d d d j (3.240)
- 51. 3.7 Solution of composite with elliptic fiber 103 (1) T (2) (2) 1 2 1 2 1 2 2[( ) ( )j j jis A M M A s M M A r 1 1 1 2 2 2 3 1 1 2 2 2 3( ) ( )]j j j j jG G G i G G GM c c c d d d j , t t (3.241) where (k=1,2) (3.242) 1 1 T T ( ) 2 , (2 ) k k k k k k k k k k k i i i i M B A H I S H A A S A B I For the case of remote heat flow, the related general solution can be obtained similarly. Set (3.243) 3 ( ) ( ) ( ) ( ) 1 2Re ( ) ( )j j j j j j k k j j k gU A F q c (3.244) 3 ( ) ( ) ( ) ( ) 1 2Re ( ) ( )j j j j j j k k j j k gB F q d where ( ) ( ) ( ) 1 ( ) lnj j j mF , 2( ) ( ) ( )2 ( ) ( ) ( ) 2 3( ) , ( )j j j j j j m m F F ( j=1, 2) (3.245) The interface condition (3.187)3,4 leads to (1) (1) * (1) * * 1 1 1 1 1 1 2 0 1 0 1 1 1 2 1 2 1 2 1 2[ ( )]( ) (a q a q c cq A A B B 1)A c B d (3.246) (2) (1) * (1) * * 1 1 1 1 1 1 2 0 1 0 1 1 1 1 2 1 2 1 1 1[ ( )]( ) (a q a q c cq A A B B 1)B d A c (3.247) (1) 1 1 1 1 1 (2) 2 1 1 1 1 1 2 1 2( ) [(q A A B B A A B B q2) 1 1 (2) 1 * 1 1 2 1 2 3 1 1 1 2( )A A B B q A * ]g B g (3.248) (2) 1 (2) (2) * 2 2 2 2 3(q A A q G c2 ) (3.249) (1) 1 1 1 1 1 (2) 3 1 1 1 1 1 2 1 2( ) [(q A A B B A A B B q3) 1 1 (2) 1 * 1 1 2 1 2 2 1 1 1 2( )A A B B q A * ]g B g (3.250) (2) 1 (2) 1 (2) 1 1 * 1 * 3 2 2 2 2 2 2 2 2 2( ) (m mq A A B B A G c B G d2 ) (3.251) where * (2) (2) (2) 1 1 2 2( mc a aG I ) (3.252)
- 52. 104 Chapter 3 Fibrous Piezoelectric Composites * (2) (2) * (1) (1) * * 1 1 1 2 1 2 2 0 1 1 2 1 1 1 0 1( ) / 2 [ (c a c a q a a c c qg c c c c) ]/ 2 (3.253) * (2) (2) * (1) (1) * * 2 1 1 2 1 2 2 0 1 1 2 1 1 1 0 1( ) / 2 [ (c a c a q a a c c qg d d d d) ]/ 2 (3.254) 3.7.3 Solutions for holes and rigid fibers When the fiber is an insulated and traction-free hole, i.e., along the hole boundary, the solutions can be found in a manner similar to that described for the piezoelectric fiber. They are 1 1 0 (1) (1) (1) (1) (1) 1 (1) (1) (1) (1) 1 1 0 1 0 0 2 0 2 0 2( ) [ ( , ) ( , )] [ ( ,t t t t t tg a q F q F a q F 0 )t (1) 1 (1) 0 1 0( ,t tq F )] (3.255) (1) (1) 1 * 1 (1) 1 1 1 2 1 1 1 1 1 12Re{ [ ( ) ( ) ] ( )}tf f p gU A P B d c (3.256) (1) (1) 1 * 1 (1) 1 1 1 2 1 1 1 1 1 12Re{ [ ( ) ( ) ] ( )}tf f p gB P B d d (3.257) for the case of a point heat source and temperature discontinuity, and (1) * (1) (1)2 (1) (1) * (1) (1) (1) (1) 2 1 0 1 2 0 1 2( ) ( / 2 ln ) ( ln / 2t t t t tg q a a q a a ) (3.258) * (1) * (1) 1 * 1 (1) 1 1 1 2 1 1 1 1 12Re{ [ ( ) ( ) ] ( )}tf f p gU A P B d c (3.259) * (1) * (1) 1 * 1 (1) 1 1 1 2 1 1 1 1 12Re{ [ ( ) ( ) ] ( )}tf f p gB P B d d ) (3.260) for the case of remote heat flow, where have, respec- tively, the same expressions as given in Eq. (3.220), except that now (1) (1) 1 2( ) and (f f ) (1) (1) 1 2( ) and ( )f f(1) (1 0q should be replaced by 0q , and * (1) * (1)2 (1) * (1) 2 (1) 1 0 0 * (1) (1) * (1) 2 (1) * (1)2 (1) 2 0 0 ( ) [ ( 2ln ) ( 2ln )]/ 4, ( ) [ ( 2ln ) ( 2ln )]/ 4 k k k k k k k k k k k k k f a q q f ibp q q (3.261) Similarly, for a rigid and nonconductive fiber, the thermal boundary condition is the same as that of a hole. However, the elastic boundary condition of the fiber should be described in a manner similar to that of Hwu and Yen [47]: 1 T 2 0 0 0( )/ 2, { , , 0, 0}ib au u u u (on the interface) (3.262) where denotes the rigid-body rotation relative to the matrix, which can be ob- tained by the condition that the total moment about the origin due to the traction along the surface of the rigid fiber vanishes.
- 53. References 105 Substituting Eqs. (3.225) (or (3.258)) and (3.262) into (3.187)3,4 provides (1) (1) 1 * 1 1 1 1 2 1 12Re{ [ ( ) ( ) ]f f pU A P A1 1c (1) (1) 1 1 1 0( ) / 2tgc }u (3.263) 1 * 1(1) (1) 1 1 1 11 2 2Re{ [ ]( ) ( ) pf fB P 1 1A c (1) 1 (1) 1 1 1 1 1 0( ) / 2tgd B A u } (3.264) for the case of a point heat source and temperature discontinuity, and 1 * 1* (1) * (1) 1 1 11 2 2Re{ [ ]( ) ( ) pf fU A P A1 1c (1) (1) 1 1 1 0( ) / 2tgc }u (3.265) 1 * 1* (1) * (1) 1 1 11 2 2Re{ [ ]( ) ( ) pf fB P 1 1A c (1) 1 (1) 1 1 1 1 1 0( ) / 2tgd B A u } k (3.266) for the case of a remote heat flow, where * * 1 1 2 1 2, , , ,k k kg f f f f have the same ex- pressions as those in Eqs. (3.255)-(3.261). Once the general solution has been ob- tained, can be determined by using the condition that the total moment about the origin due to the traction along the surface of the rigid fiber vanishes. The result is 2 T 0 T 1 0 1 1 0 2 Re{ ( ) / }d Im{ } i s ey f u B A u (3.267) where (3.268)T { sin , cos , 0, 0}b ay 1 * 1 1 1 2 1 1 1 1 1 1( ) [ ( ) ( ) ] ( )s mf f p gf B P A c d (3.269) for the case of a point heat source and temperature discontinuity, and * * 1 * 1 1 1 2 1 1 1 1 1( ) [ ( ) ( ) ] ( )s f f p gf B P A c d (3.270) for the case of a remote heat flow. References [1] He LH, Lim CW: Electromechanical responses of piezoelectric fiber composites with sliding interface under anti-plane deformations. Composites Part B: Engineering 34(4), 373-381 (2003).
- 54. 106 Chapter 3 Fibrous Piezoelectric Composites [2] Smart Material Corp. http://www.smart-material.com/. [3] Hagood NW, Kindel R, Ghandi K, Gaudenzi P: Improving transverse actuation of piezoceramics using interdigitated surface electrodes. Proc. SPIE 1917, 341-352 (1993). [4] Hagood N, Bent A: Composites for structural control. US Patent, 6048622 (2000). [5] Bent AA, Hagood NW: Improved performance in piezoelectric fibre composites using interdigitated electrodes. Proc. SPIE 2441, 196-212(1995). [6] Wilkie WK, Bryant GR, High JW, Fox RL, Hallbaum RF, Jalink A Jr, Little BD, Mirick P H: Low-cost piezocomposite actuator for structural control applications. Proc. SPIE 3991, 323(2000). [7] Cannon BJ, Brei D: Feasibility study of microfabrication by coextrusion (MFCX) hollow fibers for active composites. Journal of Intelligent Material Systems and Struc- tures 11(9), 659-670 (2000). [8] Liu HY, Qin QH, Mai YW: Theoretical model of piezoelectric fibre pull-out. Interna- tional Journal of Solids and Structures 40(20), 5511-5519 (2003). [9] Gao YC, Mai YW, Cotterell B: Fracture of fiber-reinforced materials. Zeitschrift Fur Angewandte Mathematik Und Physik 39(4), 550-572 (1988). [10] Zhou LM, Mai YW: On the single-fiber pullout and pushout problem effect of fiber anisotropy. Zeitschrift Fur Angewandte Mathematik Und Physik 44(4), 769-775 (1993). [11] Zhou LM, Kim JK, Mai YW: On the single fiber pull-out problem effect of loading method. Composites Science and Technology 45(2), 153-160 (1992). [12] Zhou LM, Kim JK, Mai YW: Interfacial debonding and fiber pull-out stresses .2. A new model based on the fracture-mechanics approach. Journal of Materials Science 27(12), 3155-3166 (1992). [13] Zhou LM, Mai YW, Ye L: Analyses of fiber push-out test based on the frac- ture-mechanics approach. Composites Engineering 5(10-11), 1199-1219 (1995). [14] Gu B, Liu HY, Mai YW: A theoretical model on piezoelectric fibre pullout with elec- tric input. Engineering Fracture Mechanics 73(14), 2053-2066 (2006). [15] Qin QH, Wang JS, Kang YL: A theoretical model for electroelastic analysis in piezo- electric fibre push-out test. Archive of Applied Mechanics 75(8-9), 527-540 (2006). [16] Wang JS, Qin QH: Debonding criterion for the piezoelectric fibre push-out test. Phi- losophical Magazine Letters 86(2), 123-136 (2006). [17] Wang JS, Qin QH, Kang YL: Stress and electric field transfer of piezoelectric fibre push-out under electric and mechanical loading. In: Ren WX, Gary Ong KC, Tan JSY (eds.) 9th International Conference on Inspection, Appraisal, Repairs & Maintenance of Structures, Fuzhou, China, 20-21 October, 2005, pp. 435-442. CI-Premier PTY LTD (2005). [18] Hill R: Elastic properties of reinforced solids: Some theoretical principles. Journal of the Mechanics and Physics of Solids 11(5), 357-372 (1963). [19] Hill R: Theory of mechanical properties of fibre-strengthened materials.1. Elastic be- haviour. Journal of the Mechanics and Physics of Solids 12(4), 199-212 (1964). [20] Grekov AA, Kramarov SO, Kuprienko AA: Effective properties of a transversely iso- tropic piezocomposite with cylindrical inclusions. Ferroelectrics 99, 115-126 (1989). [21] Dunn ML, Taya M: Micromechanics predictions of the effective electroelastic moduli
- 55. References 107 of piezoelectric composites. International Journal of Solids and Structures 30(2), 161-175 (1993). [22] Schulgasser K: Relationships between the effective properties of transversely isotropic piezoelectric composites. Journal of the Mechanics and Physics of Solids 40(2), 473-479 (1992). [23] Benveniste Y, Dvorak GJ: Uniform-fields and universal relations in piezoelectric com- posites. Journal of the Mechanics and Physics of Solids 40(6), 1295-1312 (1992). [24] Benveniste Y: Exact results in the micromechanics of fibrous piezoelectric composites exhibiting pyroelectricity. Proceedings of the Royal Society of London Series A: Mathematical Physical and Engineering Sciences 441(1911), 59-81 (1993). [25] Benveniste Y: Magnetoelectric effect in fibrous composites with piezoelectric and piezomagnetic phases. Physical Review B 51(22), 16424-16427 (1995). [26] Chen TY: Piezoelectric properties of multiphase fibrous composites some theoretical results. Journal of the Mechanics and Physics of Solids 41(11), 1781-1794 (1993). [27] Mallik N, Ray MC: Effective coefficients of piezoelectric fiber-reinforced composites. AIAA Journal 41(4), 704-710 (2003). [28] Huang JH, Kuo WS: The analysis of piezoelectric/piezomagnetic composite materials containing ellipsoidal inclusions. Journal of Applied Physics 81(3), 1378-1386 (1997). [29] Huang JH: Analytical predictions for the magnetoelectric coupling in piezomagnetic materials reinforced by piezoelectric ellipsoidal inclusions. Physical Review B 58(1), 12-15 (1998). [30] Jiang CP, Tong ZH, Cheung YK: A generalized self-consistent method for piezoelec- tric fiber reinforced composites under antiplane shear. Mechanics of Materials 33(5), 295-308 (2001). [31] Jiang CP, Tong ZH, Cheung YK: A generalized self-consistent method accounting for fiber section shape. International Journal of Solids and Structures 40(10), 2589-2609 (2003). [32] Tong ZH, Lo SH, Jiang CP, Cheung YK: An exact solution for the three-phase thermo-electro-magneto-elastic cylinder model and its application to piezoelec- tric-magnetic fiber composites. International Journal of Solids and Structures 45(20), 5205-5219 (2008). [33] Kumar A, Chakraborty D: Effective properties of thermo-electro-mechanically cou- pled piezoelectric fiber reinforced composites. Materials & Design 30(4), 1216-1222 (2009). [34] Benveniste Y: On the micromechanics of fibrous piezoelectric composites. Mechanics of Materials 18(3), 183-193 (1994). [35] Qin QH: Thermoelectroelastic solution for elliptic inclusions and application to crack-inclusion problems. Applied Mathematical Modelling 25(1), 1-23 (2000). [36] Qin QH: Fracture Mechanics of Piezoelectric Materials. WIT Press, Southampton (2001). [37] Zhang X, Liu HY, Mai YW, Diao XX: On steady-state fibre pull-out. . The stress field. Composites Science and Technology 59(15), 2179-2189 (1999). [38] Tiersten HF: Linear Piezoelectric Plate Vibrations. Plenum Press, New York (1969). [39] Zhou LM: A study on the fracture mechanics of interfaces in fibre-matrix composites. PhD Thesis, University of Sydney (1994).
- 56. 108 Chapter 3 Fibrous Piezoelectric Composites [40] Steinhausen R, Hauke T, Seifert W, Beige H, Watzka W, Seifert S, Sporn D, Starke S, Schonecker A: Finescaled piezoelectric 1-3 composites: Properties and modeling. Journal of the European Ceramic Society 19(6-7), 1289-1293 (1999). [41] Chan HLW, Li K, Choy CL: Piezoelectric ceramic fibre/epoxy 1-3 composites for high-frequency ultrasonic transducer applications. Materials Science and Engineering B: Solid State Materials for Advanced Technology 99(1-3), 29-35 (2003). [42] Nelson LJ: Smart piezoelectric fibre composites. Materials Science and Technology 18(11), 1245-1256 (2002). [43] Honda K, Kagawa Y: Debonding criterion in the pushout process of fiber-reinforced ceramics. Acta Materialia 44(8), 3267-3277 (1996). [44] Park SB, Sun CT: Effect of electric-field on fracture of piezoelectric ceramics. Interna- tional Journal of Fracture 70(3), 203-216 (1995). [45] Hashin Z: Analysis of properties of fiber composites with anisotropic constituents. Journal of Applied Mechanics-Transactions of the ASME 46(3), 543-550 (1979). [46] Ting TCT: Green’s functions for an anisotropic elliptic inclusion under generalized plane strain deformations. Quarterly Journal of Mechanics and Applied Mathematics 49, 1-18 (1996). [47] Hwu C, Yen WJ: On the anisotropic elastic inclusions in plane elastostatics. Journal of Applied Mechanics-Transactions of the ASME 60(3), 626-632 (1993). [48] Stagni L: On the elastic field perturbation by inhomogeneities in plane elasticity. Zeitschrift Fur Angewandte Mathematik Und Physik 33(3), 315-325 (1982).

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment